#------------------------------------------------------------------------------
#$Date: 2016-02-14 16:26:36 +0200 (Sun, 14 Feb 2016) $
#$Revision: 176435 $
#$URL: svn://www.crystallography.net/cod/cif/2/10/52/2105276.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2105276
loop_
_publ_author_name
'García-Tuñón, Esther'
'Dacuña, Bruno'
'Zaragoza, Guillermo'
'Franco, Jaime'
'Guitián, Francisco'
_publ_section_title
;
 Cl--OH ion-exchanging process in chlorapatite
 (Ca₅(PO₄)₃Clₓ(OH)~1{-~x}) -- a deep insight
;
_journal_coeditor_code           ZB5021
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              467
_journal_page_last               479
_journal_paper_doi               10.1107/S0108768112019520
_journal_volume                  68
_journal_year                    2012
_chemical_compound_source        'synthesis as described'
_chemical_formula_moiety         'Ca5 Cl1 O12 P3'
_chemical_formula_sum            'Ca5 Cl O12 P3'
_chemical_formula_weight         520.76
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.3
_audit_creation_date             2010-10-04T10:32:05-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                90
_cell_angle_beta                 119.9690(10)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.6307(4)
_cell_length_b                   6.7425(3)
_cell_length_c                   19.2602(7)
_cell_measurement_reflns_used    1895
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      26.34
_cell_measurement_theta_min      3.88
_cell_measurement_wavelength     0.71073
_cell_volume                     1083.44(8)
_computing_cell_refinement       'APPEX2 (BRUKER AXS, 2005)'
_computing_data_collection       'APPEX2 (BRUKER AXS, 2005)'
_computing_data_reduction        'APPEX2 (BRUKER AXS, 2005)'
_computing_molecular_graphics    'Ortep-3 for Windows (Farrugia, 1997)'
_computing_publication_material  'WinGX publication routines (Farrugia, 1999)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SIR2004 (Giacovazzo et al, 2004)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'BRUKER APPEX-II CCD'
_diffrn_measurement_method       'omega and phi scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.037
_diffrn_reflns_av_unetI/netI     0.0216
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            17423
_diffrn_reflns_theta_full        26.38
_diffrn_reflns_theta_max         26.38
_diffrn_reflns_theta_min         2.44
_exptl_absorpt_coefficient_mu    3.23
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.8695
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'BRUKER SADABS'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    3.193
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             1032
_exptl_crystal_size_max          0.17
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.116
_refine_diff_density_min         -0.587
_refine_diff_density_rms         0.119
_refine_ls_extinction_coef       0.0050(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.157
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     129
_refine_ls_number_reflns         2212
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.157
_refine_ls_R_factor_all          0.0566
_refine_ls_R_factor_gt           0.0356
_refine_ls_shift/su_max          0.028
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0339P)²+3.8081P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0841
_refine_ls_wR_factor_ref         0.0928
_reflns_number_gt                1285
_reflns_number_total             2212
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            zb5021.cif
_cod_data_source_block           A_mono
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_original_formula_sum        'Ca5 Cl1 O12 P3'
_cod_database_code               2105276
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_group
Ca1 Ca 0.74558(9) 1.25031(15) 0.00306(4) 0.00627(19) Uani 1 1 d . .
Ca2 Ca 0.66668(11) 0.99382(11) 0.16668(5) 0.0039(2) Uani 1 1 d . .
Ca3 Ca 0.66681(12) 0.50051(12) 0.16671(6) 0.0099(3) Uani 1 1 d . .
Ca4 Ca 0.26056(9) 0.25019(15) 0.12720(4) 0.00611(19) Uani 1 1 d . .
Ca5 Ca 0.00609(9) 0.75017(15) 0.13023(4) 0.00605(19) Uani 1 1 d . .
O1 O 0.9134(4) 1.0674(5) 0.1330(2) 0.0105(2) Uani 1 1 d . .
O2 O 0.8718(3) 1.2510(5) 0.23242(16) 0.0105(2) Uani 1 1 d . .
O3 O 0.5928(3) 1.2503(5) 0.06390(16) 0.0105(2) Uani 1 1 d . .
O4 O 0.3532(4) 1.0668(5) 0.0436(2) 0.0105(2) Uani 1 1 d . .
O5 O 0.5348(3) 1.2506(5) 0.20342(16) 0.0105(2) Uani 1 1 d . .
O6 O 0.7333(4) 1.0664(5) 0.3233(2) 0.0105(2) Uani 1 1 d . .
O7 O 0.6561(3) 0.7502(5) 0.07448(16) 0.0105(2) Uani 1 1 d . .
O8 O 0.8512(3) 0.7496(5) 0.25353(16) 0.0105(2) Uani 1 1 d . .
O9 O 0.4931(3) 0.7497(5) 0.17198(16) 0.0105(2) Uani 1 1 d . .
O10 O 0.9132(4) 0.4338(5) 0.1332(2) 0.0105(2) Uani 1 1 d . .
O11 O 0.7336(4) 0.4334(5) 0.3235(2) 0.0105(2) Uani 1 1 d . .
O12 O 0.3533(4) 0.4334(5) 0.0434(2) 0.0105(2) Uani 1 1 d . .
P1 P 0.96710(11) 1.2504(2) 0.18742(6) 0.0048(2) Uani 1 1 d . .
P2 P 0.40780(11) 1.2499(2) 0.01641(6) 0.0050(2) Uani 1 1 d . .
P3 P 0.62501(11) 1.25039(19) 0.29613(6) 0.0046(2) Uani 1 1 d . .
Cl1A Cl 0.0031(3) 0.5623(4) 0.00021(17) 0.0141(4) Uani 0.490(3) 1 d P 1
Cl1B Cl -0.0028(3) 0.9460(4) 0.00000(18) 0.0141(4) Uani 0.510(3) 1 d P 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.006 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Ca1 O12 87.29(12) . 3_675
O3 Ca1 O4 87.41(12) . 3_675
O12 Ca1 O4 133.10(10) 3_675 3_675
O3 Ca1 O1 75.49(11) . .
O12 Ca1 O1 140.10(12) 3_675 .
O4 Ca1 O1 82.52(12) 3_675 .
O3 Ca1 O10 75.42(11) . 1_565
O12 Ca1 O10 82.45(12) 3_675 1_565
O4 Ca1 O10 140.17(12) 3_675 1_565
O1 Ca1 O10 58.63(9) . 1_565
O3 Ca1 Cl1A 143.68(11) . 3_675
O12 Ca1 Cl1A 76.50(10) 3_675 3_675
O4 Ca1 Cl1A 127.23(10) 3_675 3_675
O1 Ca1 Cl1A 96.44(10) . 3_675
O10 Ca1 Cl1A 70.42(10) 1_565 3_675
O3 Ca1 Cl1B 143.21(11) . 3_675
O12 Ca1 Cl1B 127.91(10) 3_675 3_675
O4 Ca1 Cl1B 75.88(10) 3_675 3_675
O1 Ca1 Cl1B 70.06(10) . 3_675
O10 Ca1 Cl1B 96.73(10) 1_565 3_675
Cl1A Ca1 Cl1B 55.09(6) 3_675 3_675
O3 Ca1 O9 104.38(9) . 3_675
O12 Ca1 O9 68.21(11) 3_675 3_675
O4 Ca1 O9 68.19(11) 3_675 3_675
O1 Ca1 O9 150.63(11) . 3_675
O10 Ca1 O9 150.58(11) 1_565 3_675
Cl1A Ca1 O9 99.42(8) 3_675 3_675
Cl1B Ca1 O9 99.46(9) 3_675 3_675
O3 Ca1 P1 70.40(7) . .
O12 Ca1 P1 110.88(10) 3_675 .
O4 Ca1 P1 110.93(10) 3_675 .
O1 Ca1 P1 29.43(8) . .
O10 Ca1 P1 29.45(8) 1_565 .
Cl1A Ca1 P1 85.20(7) 3_675 .
Cl1B Ca1 P1 85.14(7) 3_675 .
O9 Ca1 P1 174.79(6) 3_675 .
O3 Ca1 Cl1B 134.01(10) . 1_655
O12 Ca1 Cl1B 138.58(10) 3_675 1_655
O4 Ca1 Cl1B 64.61(10) 3_675 1_655
O1 Ca1 Cl1B 65.71(9) . 1_655
O10 Ca1 Cl1B 102.59(9) 1_565 1_655
Cl1A Ca1 Cl1B 67.17(8) 3_675 1_655
Cl1B Ca1 Cl1B 12.08(9) 3_675 1_655
O9 Ca1 Cl1B 98.18(8) 3_675 1_655
P1 Ca1 Cl1B 85.81(6) . 1_655
O3 Ca1 Cl1A 133.90(10) . 1_665
O12 Ca1 Cl1A 64.67(10) 3_675 1_665
O4 Ca1 Cl1A 138.57(10) 3_675 1_665
O1 Ca1 Cl1A 102.46(9) . 1_665
O10 Ca1 Cl1A 65.64(9) 1_565 1_665
Cl1A Ca1 Cl1A 12.73(10) 3_675 1_665
Cl1B Ca1 Cl1A 67.82(8) 3_675 1_665
O9 Ca1 Cl1A 98.25(8) 3_675 1_665
P1 Ca1 Cl1A 85.72(6) . 1_665
Cl1B Ca1 Cl1A 79.90(5) 1_655 1_665
O3 Ca1 P2 22.50(7) . .
O12 Ca1 P2 78.80(9) 3_675 .
O4 Ca1 P2 78.84(8) 3_675 .
O1 Ca1 P2 95.04(8) . .
O10 Ca1 P2 95.00(8) 1_565 .
Cl1A Ca1 P2 152.68(7) 3_675 .
Cl1B Ca1 P2 152.02(6) 3_675 .
O9 Ca1 P2 81.89(6) 3_675 .
P1 Ca1 P2 92.90(3) . .
Cl1B Ca1 P2 139.98(6) 1_655 .
Cl1A Ca1 P2 139.98(6) 1_665 .
O7 Ca2 O9 77.66(11) . .
O7 Ca2 O8 77.67(10) . .
O9 Ca2 O8 77.67(11) . .
O7 Ca2 O3 89.86(11) . .
O9 Ca2 O3 126.49(10) . .
O8 Ca2 O3 150.09(10) . .
O7 Ca2 O2 126.55(10) . .
O9 Ca2 O2 150.13(10) . .
O8 Ca2 O2 90.01(11) . .
O3 Ca2 O2 75.65(10) . .
O7 Ca2 O5 150.04(10) . .
O9 Ca2 O5 89.98(12) . .
O8 Ca2 O5 126.63(10) . .
O3 Ca2 O5 75.61(10) . .
O2 Ca2 O5 75.60(10) . .
O7 Ca2 O6 145.67(11) . .
O9 Ca2 O6 82.09(10) . .
O8 Ca2 O6 71.06(10) . .
O3 Ca2 O6 124.43(10) . .
O2 Ca2 O6 68.14(9) . .
O5 Ca2 O6 55.78(10) . .
O7 Ca2 O4 82.17(10) . .
O9 Ca2 O4 71.00(10) . .
O8 Ca2 O4 145.66(11) . .
O3 Ca2 O4 55.71(9) . .
O2 Ca2 O4 124.28(10) . .
O5 Ca2 O4 67.96(10) . .
O6 Ca2 O4 116.87(10) . .
O7 Ca2 O1 71.04(10) . .
O9 Ca2 O1 145.68(11) . .
O8 Ca2 O1 82.16(10) . .
O3 Ca2 O1 68.05(10) . .
O2 Ca2 O1 55.73(10) . .
O5 Ca2 O1 124.29(10) . .
O6 Ca2 O1 117.04(11) . .
O4 Ca2 O1 117.01(10) . .
O7 Ca2 P2 88.53(8) . .
O9 Ca2 P2 99.44(8) . .
O8 Ca2 P2 166.19(8) . .
O3 Ca2 P2 27.56(7) . .
O2 Ca2 P2 98.47(8) . .
O5 Ca2 P2 66.45(7) . .
O6 Ca2 P2 122.22(7) . .
O4 Ca2 P2 28.44(7) . .
O1 Ca2 P2 93.59(8) . .
O7 Ca2 P1 99.43(8) . .
O9 Ca2 P1 166.25(8) . .
O8 Ca2 P1 88.58(8) . .
O3 Ca2 P1 66.52(7) . .
O2 Ca2 P1 27.62(7) . .
O5 Ca2 P1 98.50(8) . .
O6 Ca2 P1 93.70(7) . .
O4 Ca2 P1 122.23(7) . .
O1 Ca2 P1 28.40(7) . .
P2 Ca2 P1 93.88(3) . .
O7 Ca2 P3 166.31(8) . .
O9 Ca2 P3 88.65(8) . .
O8 Ca2 P3 99.50(8) . .
O3 Ca2 P3 98.51(8) . .
O2 Ca2 P3 66.43(7) . .
O5 Ca2 P3 27.64(7) . .
O6 Ca2 P3 28.45(7) . .
O4 Ca2 P3 93.57(7) . .
O1 Ca2 P3 122.15(8) . .
P2 Ca2 P3 93.89(3) . .
P1 Ca2 P3 93.85(3) . .
O9 Ca3 O8 76.77(11) . .
O9 Ca3 O7 76.66(10) . .
O8 Ca3 O7 76.70(10) . .
O9 Ca3 O2 150.10(10) . 1_545
O8 Ca3 O2 89.76(12) . 1_545
O7 Ca3 O2 126.52(10) . 1_545
O9 Ca3 O5 89.77(12) . 1_545
O8 Ca3 O5 126.55(10) . 1_545
O7 Ca3 O5 150.00(10) . 1_545
O2 Ca3 O5 76.88(10) 1_545 1_545
O9 Ca3 O3 126.39(11) . 1_545
O8 Ca3 O3 150.12(10) . 1_545
O7 Ca3 O3 89.84(11) . 1_545
O2 Ca3 O3 76.88(10) 1_545 1_545
O5 Ca3 O3 76.75(10) 1_545 1_545
O9 Ca3 O10 144.22(11) . .
O8 Ca3 O10 81.69(10) . .
O7 Ca3 O10 70.75(10) . .
O2 Ca3 O10 56.07(10) 1_545 .
O5 Ca3 O10 125.98(10) 1_545 .
O3 Ca3 O10 68.63(10) 1_545 .
O9 Ca3 O12 70.74(10) . .
O8 Ca3 O12 144.32(11) . .
O7 Ca3 O12 81.76(10) . .
O2 Ca3 O12 125.90(11) 1_545 .
O5 Ca3 O12 68.46(10) 1_545 .
O3 Ca3 O12 55.95(10) 1_545 .
O10 Ca3 O12 117.42(11) . .
O9 Ca3 O11 81.78(10) . .
O8 Ca3 O11 70.77(10) . .
O7 Ca3 O11 144.25(11) . .
O2 Ca3 O11 68.53(10) 1_545 .
O5 Ca3 O11 56.07(10) 1_545 .
O3 Ca3 O11 125.88(10) 1_545 .
O10 Ca3 O11 117.47(11) . .
O12 Ca3 O11 117.42(10) . .
O9 Ca3 P1 165.25(9) . 1_545
O8 Ca3 P1 88.50(8) . 1_545
O7 Ca3 P1 99.39(8) . 1_545
O2 Ca3 P1 27.78(7) 1_545 1_545
O5 Ca3 P1 99.85(8) 1_545 1_545
O3 Ca3 P1 67.23(7) 1_545 1_545
O10 Ca3 P1 28.65(7) . 1_545
O12 Ca3 P1 123.18(8) . 1_545
O11 Ca3 P1 94.27(7) . 1_545
O9 Ca3 P3 88.54(8) . 1_545
O8 Ca3 P3 99.37(8) . 1_545
O7 Ca3 P3 165.18(8) . 1_545
O2 Ca3 P3 67.18(7) 1_545 1_545
O5 Ca3 P3 27.82(7) 1_545 1_545
O3 Ca3 P3 99.77(8) 1_545 1_545
O10 Ca3 P3 123.26(8) . 1_545
O12 Ca3 P3 94.23(7) . 1_545
O11 Ca3 P3 28.60(7) . 1_545
P1 Ca3 P3 94.75(4) 1_545 1_545
O9 Ca3 P2 99.35(8) . 1_545
O8 Ca3 P2 165.26(8) . 1_545
O7 Ca3 P2 88.57(8) . 1_545
O2 Ca3 P2 99.78(8) 1_545 1_545
O5 Ca3 P2 67.10(7) 1_545 1_545
O3 Ca3 P2 27.69(7) 1_545 1_545
O10 Ca3 P2 94.26(8) . 1_545
O12 Ca3 P2 28.61(7) . 1_545
O11 Ca3 P2 123.16(8) . 1_545
P1 Ca3 P2 94.71(4) 1_545 1_545
P3 Ca3 P2 94.70(4) 1_545 1_545
O5 Ca4 O6 87.18(12) 1_545 2_645
O5 Ca4 O11 87.39(12) 1_545 2_645
O6 Ca4 O11 133.19(10) 2_645 2_645
O5 Ca4 O4 75.38(11) 1_545 1_545
O6 Ca4 O4 140.14(11) 2_645 1_545
O11 Ca4 O4 82.28(11) 2_645 1_545
O5 Ca4 O12 75.31(11) 1_545 .
O6 Ca4 O12 82.44(11) 2_645 .
O11 Ca4 O12 140.01(11) 2_645 .
O4 Ca4 O12 58.71(9) 1_545 .
O5 Ca4 Cl1B 142.68(11) 1_545 3_565
O6 Ca4 Cl1B 128.48(10) 2_645 3_565
O11 Ca4 Cl1B 75.72(10) 2_645 3_565
O4 Ca4 Cl1B 69.59(10) 1_545 3_565
O12 Ca4 Cl1B 96.55(10) . 3_565
O5 Ca4 Cl1A 144.18(10) 1_545 3_565
O6 Ca4 Cl1A 76.80(10) 2_645 3_565
O11 Ca4 Cl1A 126.76(10) 2_645 3_565
O4 Ca4 Cl1A 96.73(10) 1_545 3_565
O12 Ca4 Cl1A 71.00(9) . 3_565
Cl1B Ca4 Cl1A 55.03(6) 3_565 3_565
O5 Ca4 O8 104.49(9) 1_545 2_645
O6 Ca4 O8 68.32(11) 2_645 2_645
O11 Ca4 O8 68.25(11) 2_645 2_645
O4 Ca4 O8 150.45(11) 1_545 2_645
O12 Ca4 O8 150.67(11) . 2_645
Cl1B Ca4 O8 99.78(8) 3_565 2_645
Cl1A Ca4 O8 99.04(8) 3_565 2_645
O5 Ca4 P2 70.35(7) 1_545 1_545
O6 Ca4 P2 110.89(9) 2_645 1_545
O11 Ca4 P2 110.76(9) 2_645 1_545
O4 Ca4 P2 29.48(8) 1_545 1_545
O12 Ca4 P2 29.47(8) . 1_545
Cl1B Ca4 P2 84.71(6) 3_565 1_545
Cl1A Ca4 P2 85.61(6) 3_565 1_545
O8 Ca4 P2 174.84(6) 2_645 1_545
O5 Ca4 Cl1B 134.70(10) 1_545 1_545
O6 Ca4 Cl1B 138.00(10) 2_645 1_545
O11 Ca4 Cl1B 64.93(10) 2_645 1_545
O4 Ca4 Cl1B 66.31(9) 1_545 1_545
O12 Ca4 Cl1B 102.74(10) . 1_545
Cl1B Ca4 Cl1B 11.26(10) 3_565 1_545
Cl1A Ca4 Cl1B 66.25(8) 3_565 1_545
O8 Ca4 Cl1B 97.73(8) 2_645 1_545
P2 Ca4 Cl1B 86.18(5) 1_545 1_545
O5 Ca4 Cl1A 133.22(10) 1_545 .
O6 Ca4 Cl1A 64.34(10) 2_645 .
O11 Ca4 Cl1A 139.26(10) 2_645 .
O4 Ca4 Cl1A 102.60(9) 1_545 .
O12 Ca4 Cl1A 65.24(9) . .
Cl1B Ca4 Cl1A 68.69(8) 3_565 .
Cl1A Ca4 Cl1A 13.69(10) 3_565 .
O8 Ca4 Cl1A 98.49(8) 2_645 .
P2 Ca4 Cl1A 85.48(5) 1_545 .
Cl1B Ca4 Cl1A 79.93(5) 1_545 .
O5 Ca4 P3 22.54(7) 1_545 1_545
O6 Ca4 P3 78.69(9) 2_645 1_545
O11 Ca4 P3 78.84(9) 2_645 1_545
O4 Ca4 P3 94.94(8) 1_545 1_545
O12 Ca4 P3 94.93(8) . 1_545
Cl1B Ca4 P3 151.67(7) 3_565 1_545
Cl1A Ca4 P3 153.07(7) 3_565 1_545
O8 Ca4 P3 81.95(6) 2_645 1_545
P2 Ca4 P3 92.89(3) 1_545 1_545
Cl1B Ca4 P3 140.56(6) 1_545 1_545
Cl1A Ca4 P3 139.38(6) . 1_545
O2 Ca5 O10 87.47(13) 2_645 1_455
O2 Ca5 O1 87.29(13) 2_645 1_455
O10 Ca5 O1 133.28(10) 1_455 1_455
O2 Ca5 O11 75.25(11) 2_645 2_655
O10 Ca5 O11 140.06(12) 1_455 2_655
O1 Ca5 O11 82.36(11) 1_455 2_655
O2 Ca5 O6 75.32(11) 2_645 2_645
O10 Ca5 O6 82.40(11) 1_455 2_645
O1 Ca5 O6 140.01(12) 1_455 2_645
O11 Ca5 O6 58.64(9) 2_655 2_645
O2 Ca5 Cl1A 143.49(10) 2_645 .
O10 Ca5 Cl1A 76.95(10) 1_455 .
O1 Ca5 Cl1A 127.22(11) 1_455 .
O11 Ca5 Cl1A 95.84(9) 2_655 .
O6 Ca5 Cl1A 70.06(10) 2_645 .
O2 Ca5 Cl1B 143.16(11) 2_645 .
O10 Ca5 Cl1B 127.96(11) 1_455 .
O1 Ca5 Cl1B 75.35(10) 1_455 .
O11 Ca5 Cl1B 70.46(10) 2_655 .
O6 Ca5 Cl1B 97.41(10) 2_645 .
Cl1A Ca5 Cl1B 55.13(6) . .
O2 Ca5 O7 104.55(9) 2_645 1_455
O10 Ca5 O7 68.26(11) 1_455 1_455
O1 Ca5 O7 68.34(11) 1_455 1_455
O11 Ca5 O7 150.61(11) 2_655 1_455
O6 Ca5 O7 150.57(11) 2_645 1_455
Cl1A Ca5 O7 100.00(8) . 1_455
Cl1B Ca5 O7 98.87(8) . 1_455
O2 Ca5 P3 70.26(7) 2_645 2_645
O10 Ca5 P3 110.88(9) 1_455 2_645
O1 Ca5 P3 110.74(9) 1_455 2_645
O11 Ca5 P3 29.40(8) 2_655 2_645
O6 Ca5 P3 29.49(8) 2_645 2_645
Cl1A Ca5 P3 84.64(6) . 2_645
Cl1B Ca5 P3 85.68(6) . 2_645
O7 Ca5 P3 174.81(6) 1_455 2_645
O2 Ca5 Cl1B 133.99(11) 2_645 3_575
O10 Ca5 Cl1B 138.35(11) 1_455 3_575
O1 Ca5 Cl1B 65.16(10) 1_455 3_575
O11 Ca5 Cl1B 65.54(10) 2_655 3_575
O6 Ca5 Cl1B 102.06(9) 2_645 3_575
Cl1A Ca5 Cl1B 66.38(8) . 3_575
Cl1B Ca5 Cl1B 11.30(10) . 3_575
O7 Ca5 Cl1B 98.60(8) 1_455 3_575
P3 Ca5 Cl1B 85.37(6) 2_645 3_575
O2 Ca5 Cl1A 133.90(11) 2_645 3_565
O10 Ca5 Cl1A 63.97(10) 1_455 3_565
O1 Ca5 Cl1A 138.73(11) 1_455 3_565
O11 Ca5 Cl1A 103.24(9) 2_655 3_565
O6 Ca5 Cl1A 66.07(9) 2_645 3_565
Cl1A Ca5 Cl1A 13.55(10) . 3_565
Cl1B Ca5 Cl1A 68.63(8) . 3_565
O7 Ca5 Cl1A 97.60(8) 1_455 3_565
P3 Ca5 Cl1A 86.35(5) 2_645 3_565
Cl1B Ca5 Cl1A 79.90(5) 3_575 3_565
O2 Ca5 P1 22.56(7) 2_645 2_645
O10 Ca5 P1 78.83(9) 1_455 2_645
O1 Ca5 P1 78.88(9) 1_455 2_645
O11 Ca5 P1 94.93(8) 2_655 2_645
O6 Ca5 P1 94.88(8) 2_645 2_645
Cl1A Ca5 P1 152.89(7) . 2_645
Cl1B Ca5 P1 151.75(7) . 2_645
O7 Ca5 P1 81.98(6) 1_455 2_645
P3 Ca5 P1 92.82(3) 2_645 2_645
Cl1B Ca5 P1 140.45(6) 3_575 2_645
Cl1A Ca5 P1 139.51(6) 3_565 2_645
P1 O1 Ca5 138.9(2) . 1_655
P1 O1 Ca1 96.59(15) . .
Ca5 O1 Ca1 119.29(14) 1_655 .
P1 O1 Ca2 91.16(15) . .
Ca5 O1 Ca2 102.83(11) 1_655 .
Ca1 O1 Ca2 96.84(11) . .
P1 O2 Ca5 122.68(15) . 2_655
P1 O2 Ca3 105.48(16) . 1_565
Ca5 O2 Ca3 114.81(13) 2_655 1_565
P1 O2 Ca2 105.04(16) . .
Ca5 O2 Ca2 114.22(13) 2_655 .
Ca3 O2 Ca2 89.16(9) 1_565 .
P2 O3 Ca1 122.84(15) . .
P2 O3 Ca3 105.49(16) . 1_565
Ca1 O3 Ca3 114.56(13) . 1_565
P2 O3 Ca2 105.14(16) . .
Ca1 O3 Ca2 114.26(13) . .
Ca3 O3 Ca2 89.03(9) 1_565 .
P2 O4 Ca1 138.6(2) . 3_675
P2 O4 Ca4 96.57(15) . 1_565
Ca1 O4 Ca4 119.36(13) 3_675 1_565
P2 O4 Ca2 91.25(15) . .
Ca1 O4 Ca2 103.02(12) 3_675 .
Ca4 O4 Ca2 96.99(12) 1_565 .
P3 O5 Ca4 122.85(15) . 1_565
P3 O5 Ca3 105.30(16) . 1_565
Ca4 O5 Ca3 114.78(13) 1_565 1_565
P3 O5 Ca2 105.02(16) . .
Ca4 O5 Ca2 114.30(13) 1_565 .
Ca3 O5 Ca2 89.06(9) 1_565 .
P3 O6 Ca4 139.05(19) . 2_655
P3 O6 Ca5 96.30(15) . 2_655
Ca4 O6 Ca5 119.13(14) 2_655 2_655
P3 O6 Ca2 91.32(16) . .
Ca4 O6 Ca2 103.13(12) 2_655 .
Ca5 O6 Ca2 96.88(11) 2_655 .
P2 O7 Ca2 133.8(2) 3_675 .
P2 O7 Ca3 133.1(2) 3_675 .
Ca2 O7 Ca3 87.83(9) . .
P2 O7 Ca5 98.49(12) 3_675 1_655
Ca2 O7 Ca5 96.43(10) . 1_655
Ca3 O7 Ca5 96.32(10) . 1_655
P1 O8 Ca2 133.6(2) 2_745 .
P1 O8 Ca3 133.4(2) 2_745 .
Ca2 O8 Ca3 87.81(9) . .
P1 O8 Ca4 98.35(12) 2_745 2_655
Ca2 O8 Ca4 96.31(10) . 2_655
Ca3 O8 Ca4 96.36(10) . 2_655
P3 O9 Ca2 133.5(2) 2_645 .
P3 O9 Ca3 133.3(2) 2_645 .
Ca2 O9 Ca3 87.89(9) . .
P3 O9 Ca1 98.34(13) 2_645 3_675
Ca2 O9 Ca1 96.46(10) . 3_675
Ca3 O9 Ca1 96.41(10) . 3_675
P1 O10 Ca5 138.9(2) 1_545 1_655
P1 O10 Ca1 96.43(15) 1_545 1_545
Ca5 O10 Ca1 119.23(14) 1_655 1_545
P1 O10 Ca3 90.56(15) 1_545 .
Ca5 O10 Ca3 103.88(12) 1_655 .
Ca1 O10 Ca3 96.46(11) 1_545 .
P3 O11 Ca4 138.94(19) 1_545 2_655
P3 O11 Ca5 96.55(15) 1_545 2_645
Ca4 O11 Ca5 119.20(14) 2_655 2_645
P3 O11 Ca3 90.52(16) 1_545 .
Ca4 O11 Ca3 103.76(12) 2_655 .
Ca5 O11 Ca3 96.45(11) 2_645 .
P2 O12 Ca1 138.9(2) 1_545 3_675
P2 O12 Ca4 96.46(15) 1_545 .
Ca1 O12 Ca4 119.18(13) 3_675 .
P2 O12 Ca3 90.65(15) 1_545 .
Ca1 O12 Ca3 103.88(12) 3_675 .
Ca4 O12 Ca3 96.50(12) . .
O10 P1 O1 107.49(15) 1_565 .
O10 P1 O8 112.30(19) 1_565 2_755
O1 P1 O8 111.94(19) . 2_755
O10 P1 O2 106.65(19) 1_565 .
O1 P1 O2 107.05(19) . .
O8 P1 O2 111.11(15) 2_755 .
O10 P1 Ca1 54.12(13) 1_565 .
O1 P1 Ca1 53.98(13) . .
O8 P1 Ca1 136.50(11) 2_755 .
O2 P1 Ca1 112.39(11) . .
O10 P1 Ca3 60.79(13) 1_565 1_565
O1 P1 Ca3 111.37(13) . 1_565
O8 P1 Ca3 135.90(14) 2_755 1_565
O2 P1 Ca3 46.74(12) . 1_565
Ca1 P1 Ca3 78.16(3) . 1_565
O10 P1 Ca2 111.83(13) 1_565 .
O1 P1 Ca2 60.44(13) . .
O8 P1 Ca2 135.19(14) 2_755 .
O2 P1 Ca2 47.34(13) . .
Ca1 P1 Ca2 78.23(3) . .
Ca3 P1 Ca2 64.34(3) 1_565 .
O10 P1 Ca5 122.08(14) 1_565 2_655
O1 P1 Ca5 122.20(14) . 2_655
O8 P1 Ca5 76.36(11) 2_755 2_655
Ca1 P1 Ca5 147.14(4) . 2_655
Ca3 P1 Ca5 74.06(3) 1_565 2_655
Ca2 P1 Ca5 74.16(3) . 2_655
O10 P1 Ca4 80.29(13) 1_565 1_665
O1 P1 Ca4 80.12(13) . 1_665
O8 P1 Ca4 56.27(10) 2_755 1_665
O2 P1 Ca4 167.37(11) . 1_665
Ca1 P1 Ca4 80.23(3) . 1_665
Ca3 P1 Ca4 141.05(5) 1_565 1_665
Ca2 P1 Ca4 140.51(5) . 1_665
Ca5 P1 Ca4 132.62(3) 2_655 1_665
O12 P2 O4 107.45(15) 1_565 .
O12 P2 O7 112.1(2) 1_565 3_675
O4 P2 O7 112.2(2) . 3_675
O12 P2 O3 106.68(19) 1_565 .
O4 P2 O3 106.86(19) . .
O7 P2 O3 111.22(15) 3_675 .
O12 P2 Ca4 54.08(13) 1_565 1_565
O4 P2 Ca4 53.95(13) . 1_565
O7 P2 Ca4 136.34(11) 3_675 1_565
O3 P2 Ca4 112.45(11) . 1_565
O12 P2 Ca3 60.74(14) 1_565 1_565
O4 P2 Ca3 111.18(14) . 1_565
O7 P2 Ca3 135.86(14) 3_675 1_565
O3 P2 Ca3 46.82(12) . 1_565
Ca4 P2 Ca3 78.15(3) 1_565 1_565
O12 P2 Ca2 111.75(14) 1_565 .
O4 P2 Ca2 60.31(14) . .
O7 P2 Ca2 135.45(14) 3_675 .
O3 P2 Ca2 47.29(12) . .
Ca4 P2 Ca2 78.25(3) 1_565 .
Ca3 P2 Ca2 64.30(3) 1_565 .
O12 P2 Ca1 121.97(13) 1_565 .
O4 P2 Ca1 122.19(13) . .
O7 P2 Ca1 76.55(11) 3_675 .
Ca4 P2 Ca1 147.11(4) 1_565 .
Ca3 P2 Ca1 73.99(3) 1_565 .
Ca2 P2 Ca1 74.15(3) . .
O12 P2 Ca5 80.30(14) 1_565 3_575
O4 P2 Ca5 80.29(14) . 3_575
O7 P2 Ca5 56.15(10) 3_675 3_575
O3 P2 Ca5 167.36(11) . 3_575
Ca4 P2 Ca5 80.19(3) 1_565 3_575
Ca3 P2 Ca5 141.01(4) 1_565 3_575
Ca2 P2 Ca5 140.55(4) . 3_575
Ca1 P2 Ca5 132.70(3) . 3_575
O11 P3 O6 107.67(15) 1_565 .
O11 P3 O9 112.24(19) 1_565 2_655
O6 P3 O9 111.91(19) . 2_655
O11 P3 O5 106.87(19) 1_565 .
O6 P3 O5 106.78(19) . .
O9 P3 O5 111.07(15) 2_655 .
O11 P3 Ca5 54.06(13) 1_565 2_655
O6 P3 Ca5 54.21(13) . 2_655
O9 P3 Ca5 136.41(11) 2_655 2_655
O5 P3 Ca5 112.52(11) . 2_655
O11 P3 Ca3 60.87(14) 1_565 1_565
O6 P3 Ca3 111.32(13) . 1_565
O9 P3 Ca3 135.94(14) 2_655 1_565
O5 P3 Ca3 46.88(12) . 1_565
Ca5 P3 Ca3 78.17(3) 2_655 1_565
O11 P3 Ca2 111.85(13) 1_565 .
O6 P3 Ca2 60.23(14) . .
O9 P3 Ca2 135.25(14) 2_655 .
O5 P3 Ca2 47.34(12) . .
Ca5 P3 Ca2 78.25(3) 2_655 .
Ca3 P3 Ca2 64.33(3) 1_565 .
O11 P3 Ca4 122.18(14) 1_565 1_565
O6 P3 Ca4 121.88(14) . 1_565
O9 P3 Ca4 76.46(11) 2_655 1_565
Ca5 P3 Ca4 147.13(4) 2_655 1_565
Ca3 P3 Ca4 74.05(3) 1_565 1_565
Ca2 P3 Ca4 74.12(3) . 1_565
O11 P3 Ca1 80.21(14) 1_565 4_586
O6 P3 Ca1 80.25(14) . 4_586
O9 P3 Ca1 56.26(11) 2_655 4_586
O5 P3 Ca1 167.33(11) . 4_586
Ca5 P3 Ca1 80.15(3) 2_655 4_586
Ca3 P3 Ca1 141.06(4) 1_565 4_586
Ca2 P3 Ca1 140.44(4) . 4_586
Ca4 P3 Ca1 132.72(3) 1_565 4_586
Cl1A Cl1A Ca1 121.1(4) 3_565 3_675
Cl1A Cl1A Ca5 115.4(4) 3_565 .
Ca1 Cl1A Ca5 101.34(9) 3_675 .
Cl1A Cl1A Ca4 114.4(4) 3_565 3_565
Ca1 Cl1A Ca4 101.26(9) 3_675 3_565
Ca5 Cl1A Ca4 100.34(8) . 3_565
Cl1A Cl1A Ca4 51.9(4) 3_565 .
Ca1 Cl1A Ca4 88.02(7) 3_675 .
Ca5 Cl1A Ca4 87.50(8) . .
Ca4 Cl1A Ca4 166.31(10) 3_565 .
Cl1A Cl1A Ca5 51.0(3) 3_565 3_565
Ca1 Cl1A Ca5 87.98(7) 3_675 3_565
Ca5 Cl1A Ca5 166.45(10) . 3_565
Ca4 Cl1A Ca5 87.28(8) 3_565 3_565
Ca4 Cl1A Ca5 82.96(6) . 3_565
Cl1A Cl1A Ca1 46.2(3) 3_565 1_445
Ca1 Cl1A Ca1 167.27(10) 3_675 1_445
Ca5 Cl1A Ca1 86.84(7) . 1_445
Ca4 Cl1A Ca1 86.66(7) 3_565 1_445
Ca4 Cl1A Ca1 82.55(6) . 1_445
Ca5 Cl1A Ca1 82.41(6) 3_565 1_445
Cl1B Cl1B Ca4 120.3(5) 3_575 3_565
Cl1B Cl1B Ca5 120.1(5) 3_575 .
Ca4 Cl1B Ca5 100.26(8) 3_565 .
Cl1B Cl1B Ca1 113.6(4) 3_575 3_675
Ca4 Cl1B Ca1 99.40(9) 3_565 3_675
Ca5 Cl1B Ca1 99.36(9) . 3_675
Cl1B Cl1B Ca1 54.3(4) 3_575 1_455
Ca4 Cl1B Ca1 88.30(8) 3_565 1_455
Ca5 Cl1B Ca1 88.30(7) . 1_455
Ca1 Cl1B Ca1 167.92(9) 3_675 1_455
Cl1B Cl1B Ca5 48.6(4) 3_575 3_575
Ca4 Cl1B Ca5 87.69(8) 3_565 3_575
Ca5 Cl1B Ca5 168.70(10) . 3_575
Ca1 Cl1B Ca5 87.12(7) 3_675 3_575
Ca1 Cl1B Ca5 83.89(7) 1_455 3_575
Cl1B Cl1B Ca4 48.5(4) 3_575 1_565
Ca4 Cl1B Ca4 168.74(10) 3_565 1_565
Ca5 Cl1B Ca4 87.65(8) . 1_565
Ca1 Cl1B Ca4 87.08(7) 3_675 1_565
Ca1 Cl1B Ca4 83.90(7) 1_455 1_565
Ca5 Cl1B Ca4 83.42(6) 3_575 1_565
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ca1 O3 2.294(3) .
Ca1 O12 2.325(3) 3_675
Ca1 O4 2.330(3) 3_675
Ca1 O1 2.522(4) .
Ca1 O10 2.525(4) 1_565
Ca1 Cl1A 2.758(3) 3_675
Ca1 Cl1B 2.835(3) 3_675
Ca1 O9 2.984(3) 3_675
Ca1 P1 3.0970(12) .
Ca1 Cl1B 3.198(3) 1_655
Ca1 Cl1A 3.274(3) 1_665
Ca1 P2 3.3889(12) .
Ca2 O7 2.384(3) .
Ca2 O9 2.384(3) .
Ca2 O8 2.387(3) .
Ca2 O3 2.451(3) .
Ca2 O2 2.452(3) .
Ca2 O5 2.452(3) .
Ca2 O6 2.796(4) .
Ca2 O4 2.798(4) .
Ca2 O1 2.802(3) .
Ca2 P2 3.2196(14) .
Ca2 P1 3.2201(14) .
Ca2 P3 3.2202(13) .
Ca3 O9 2.409(3) .
Ca3 O8 2.409(3) .
Ca3 O7 2.412(3) .
Ca3 O2 2.415(3) 1_545
Ca3 O5 2.420(3) 1_545
Ca3 O3 2.422(3) 1_545
Ca3 O10 2.790(3) .
Ca3 O12 2.792(4) .
Ca3 O11 2.793(4) .
Ca3 P1 3.1960(14) 1_545
Ca3 P3 3.1972(14) 1_545
Ca3 P2 3.2004(14) 1_545
Ca4 O5 2.293(3) 1_545
Ca4 O6 2.324(3) 2_645
Ca4 O11 2.326(3) 2_645
Ca4 O4 2.520(3) 1_545
Ca4 O12 2.524(3) .
Ca4 Cl1B 2.800(3) 3_565
Ca4 Cl1A 2.800(3) 3_565
Ca4 O8 2.984(3) 2_645
Ca4 P2 3.0963(11) 1_545
Ca4 Cl1B 3.230(3) 1_545
Ca4 Cl1A 3.240(3) .
Ca4 P3 3.3906(12) 1_545
Ca5 O2 2.296(3) 2_645
Ca5 O10 2.325(3) 1_455
Ca5 O1 2.329(3) 1_455
Ca5 O11 2.525(3) 2_655
Ca5 O6 2.528(3) 2_645
Ca5 Cl1A 2.794(3) .
Ca5 Cl1B 2.798(3) .
Ca5 O7 2.983(3) 1_455
Ca5 P3 3.0983(12) 2_645
Ca5 Cl1B 3.226(3) 3_575
Ca5 Cl1A 3.246(3) 3_565
Ca5 P1 3.3906(12) 2_645
O1 P1 1.532(3) .
O1 Ca5 2.329(3) 1_655
O2 P1 1.546(3) .
O2 Ca5 2.296(3) 2_655
O2 Ca3 2.415(3) 1_565
O3 P2 1.543(3) .
O3 Ca3 2.422(3) 1_565
O4 P2 1.534(3) .
O4 Ca1 2.330(3) 3_675
O4 Ca4 2.520(3) 1_565
O5 P3 1.547(3) .
O5 Ca4 2.293(3) 1_565
O5 Ca3 2.420(3) 1_565
O6 P3 1.534(3) .
O6 Ca4 2.324(3) 2_655
O6 Ca5 2.528(3) 2_655
O7 P2 1.538(3) 3_675
O7 Ca5 2.983(3) 1_655
O8 P1 1.538(3) 2_745
O8 Ca4 2.984(3) 2_655
O9 P3 1.539(3) 2_645
O9 Ca1 2.984(3) 3_675
O10 P1 1.532(3) 1_545
O10 Ca5 2.325(3) 1_655
O10 Ca1 2.525(4) 1_545
O11 P3 1.531(3) 1_545
O11 Ca4 2.326(3) 2_655
O11 Ca5 2.525(3) 2_645
O12 P2 1.533(3) 1_545
O12 Ca1 2.325(3) 3_675
P1 O10 1.532(3) 1_565
P1 O8 1.538(3) 2_755
P1 Ca3 3.1960(14) 1_565
P1 Ca5 3.3906(12) 2_655
P2 O12 1.533(3) 1_565
P2 O7 1.538(3) 3_675
P2 Ca4 3.0963(11) 1_565
P2 Ca3 3.2004(14) 1_565
P3 O11 1.531(3) 1_565
P3 O9 1.539(3) 2_655
P3 Ca5 3.0983(12) 2_655
P3 Ca3 3.1972(14) 1_565
P3 Ca4 3.3906(12) 1_565
Cl1A Cl1A 0.842(5) 3_565
Cl1A Ca1 2.758(3) 3_675
Cl1A Ca4 2.800(3) 3_565
Cl1A Ca5 3.246(3) 3_565
Cl1A Ca1 3.274(3) 1_445
Cl1B Cl1B 0.730(5) 3_575
Cl1B Ca4 2.800(3) 3_565
Cl1B Ca1 2.835(3) 3_675
Cl1B Ca1 3.198(3) 1_455
Cl1B Ca5 3.226(3) 3_575
Cl1B Ca4 3.230(3) 1_565
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O3 Ca1 O1 P1 -75.75(16) . .
O12 Ca1 O1 P1 -8.4(3) 3_675 .
O4 Ca1 O1 P1 -164.99(16) 3_675 .
O10 Ca1 O1 P1 5.82(10) 1_565 .
Cl1A Ca1 O1 P1 68.19(15) 3_675 .
Cl1B Ca1 O1 P1 117.37(16) 3_675 .
O9 Ca1 O1 P1 -169.37(12) 3_675 .
Cl1B Ca1 O1 P1 129.55(17) 1_655 .
Cl1A Ca1 O1 P1 56.81(15) 1_665 .
P2 Ca1 O1 P1 -86.97(14) . .
O3 Ca1 O1 Ca5 125.12(17) . 1_655
O12 Ca1 O1 Ca5 -167.57(14) 3_675 1_655
O4 Ca1 O1 Ca5 35.87(15) 3_675 1_655
O10 Ca1 O1 Ca5 -153.3(2) 1_565 1_655
Cl1A Ca1 O1 Ca5 -90.95(15) 3_675 1_655
Cl1B Ca1 O1 Ca5 -41.76(13) 3_675 1_655
O9 Ca1 O1 Ca5 31.5(3) 3_675 1_655
P1 Ca1 O1 Ca5 -159.1(3) . 1_655
Cl1B Ca1 O1 Ca5 -29.59(12) 1_655 1_655
Cl1A Ca1 O1 Ca5 -102.32(14) 1_665 1_655
P2 Ca1 O1 Ca5 113.89(14) . 1_655
O3 Ca1 O1 Ca2 16.22(11) . .
O12 Ca1 O1 Ca2 83.54(18) 3_675 .
O4 Ca1 O1 Ca2 -73.02(11) 3_675 .
O10 Ca1 O1 Ca2 97.79(14) 1_565 .
Cl1A Ca1 O1 Ca2 160.16(9) 3_675 .
Cl1B Ca1 O1 Ca2 -150.66(11) 3_675 .
O9 Ca1 O1 Ca2 -77.4(2) 3_675 .
P1 Ca1 O1 Ca2 91.97(16) . .
Cl1B Ca1 O1 Ca2 -138.49(12) 1_655 .
Cl1A Ca1 O1 Ca2 148.78(8) 1_665 .
P2 Ca1 O1 Ca2 5.00(9) . .
O7 Ca2 O1 P1 178.73(18) . .
O9 Ca2 O1 P1 -155.93(15) . .
O8 Ca2 O1 P1 -101.68(16) . .
O3 Ca2 O1 P1 80.94(15) . .
O2 Ca2 O1 P1 -6.28(13) . .
O5 Ca2 O1 P1 27.7(2) . .
O6 Ca2 O1 P1 -37.66(18) . .
O4 Ca2 O1 P1 108.41(15) . .
P2 Ca2 O1 P1 91.53(14) . .
P3 Ca2 O1 P1 -5.35(18) . .
O7 Ca2 O1 Ca5 -40.23(12) . 1_655
O9 Ca2 O1 Ca5 -14.9(3) . 1_655
O8 Ca2 O1 Ca5 39.36(13) . 1_655
O3 Ca2 O1 Ca5 -138.03(15) . 1_655
O2 Ca2 O1 Ca5 134.76(17) . 1_655
O5 Ca2 O1 Ca5 168.78(10) . 1_655
O6 Ca2 O1 Ca5 103.38(13) . 1_655
O4 Ca2 O1 Ca5 -110.56(13) . 1_655
P2 Ca2 O1 Ca5 -127.44(11) . 1_655
P1 Ca2 O1 Ca5 141.0(2) . 1_655
P3 Ca2 O1 Ca5 135.69(9) . 1_655
O7 Ca2 O1 Ca1 81.96(12) . .
O9 Ca2 O1 Ca1 107.30(17) . .
O8 Ca2 O1 Ca1 161.55(12) . .
O3 Ca2 O1 Ca1 -15.84(10) . .
O2 Ca2 O1 Ca1 -103.05(14) . .
O5 Ca2 O1 Ca1 -69.03(14) . .
O6 Ca2 O1 Ca1 -134.44(10) . .
O4 Ca2 O1 Ca1 11.63(14) . .
P2 Ca2 O1 Ca1 -5.25(9) . .
P1 Ca2 O1 Ca1 -96.78(16) . .
P3 Ca2 O1 Ca1 -102.12(10) . .
O7 Ca2 O2 P1 12.3(2) . .
O9 Ca2 O2 P1 151.55(18) . .
O8 Ca2 O2 P1 86.93(16) . .
O3 Ca2 O2 P1 -66.54(16) . .
O5 Ca2 O2 P1 -145.05(18) . .
O6 Ca2 O2 P1 156.46(19) . .
O4 Ca2 O2 P1 -95.13(18) . .
O1 Ca2 O2 P1 6.44(13) . .
P2 Ca2 O2 P1 -82.13(15) . .
P3 Ca2 O2 P1 -172.70(18) . .
O7 Ca2 O2 Ca5 -124.88(14) . 2_655
O9 Ca2 O2 Ca5 14.3(3) . 2_655
O8 Ca2 O2 Ca5 -50.29(14) . 2_655
O3 Ca2 O2 Ca5 156.24(15) . 2_655
O5 Ca2 O2 Ca5 77.73(14) . 2_655
O6 Ca2 O2 Ca5 19.24(12) . 2_655
O4 Ca2 O2 Ca5 127.65(13) . 2_655
O1 Ca2 O2 Ca5 -130.78(18) . 2_655
P2 Ca2 O2 Ca5 140.65(11) . 2_655
P1 Ca2 O2 Ca5 -137.2(3) . 2_655
P3 Ca2 O2 Ca5 50.08(10) . 2_655
O7 Ca2 O2 Ca3 118.15(12) . 1_565
O9 Ca2 O2 Ca3 -102.6(2) . 1_565
O8 Ca2 O2 Ca3 -167.26(10) . 1_565
O3 Ca2 O2 Ca3 39.27(9) . 1_565
O5 Ca2 O2 Ca3 -39.25(9) . 1_565
O6 Ca2 O2 Ca3 -97.74(11) . 1_565
O4 Ca2 O2 Ca3 10.68(14) . 1_565
O1 Ca2 O2 Ca3 112.25(13) . 1_565
P2 Ca2 O2 Ca3 23.67(8) . 1_565
P1 Ca2 O2 Ca3 105.81(17) . 1_565
P3 Ca2 O2 Ca3 -66.89(7) . 1_565
O12 Ca1 O3 P2 66.8(2) 3_675 .
O4 Ca1 O3 P2 -66.6(2) 3_675 .
O1 Ca1 O3 P2 -149.5(3) . .
O10 Ca1 O3 P2 149.7(3) 1_565 .
Cl1A Ca1 O3 P2 129.5(2) 3_675 .
Cl1B Ca1 O3 P2 -128.7(2) 3_675 .
O9 Ca1 O3 P2 0.1(3) 3_675 .
P1 Ca1 O3 P2 -179.9(3) . .
Cl1B Ca1 O3 P2 -116.8(2) 1_655 .
Cl1A Ca1 O3 P2 117.0(2) 1_665 .
O12 Ca1 O3 Ca3 -63.32(15) 3_675 1_565
O4 Ca1 O3 Ca3 163.29(15) 3_675 1_565
O1 Ca1 O3 Ca3 80.34(14) . 1_565
O10 Ca1 O3 Ca3 19.58(13) 1_565 1_565
Cl1A Ca1 O3 Ca3 -0.6(3) 3_675 1_565
Cl1B Ca1 O3 Ca3 101.2(2) 3_675 1_565
O9 Ca1 O3 Ca3 -130.01(13) 3_675 1_565
P1 Ca1 O3 Ca3 49.98(10) . 1_565
Cl1B Ca1 O3 Ca3 113.12(15) 1_655 1_565
Cl1A Ca1 O3 Ca3 -13.1(2) 1_665 1_565
P2 Ca1 O3 Ca3 -130.1(3) . 1_565
O12 Ca1 O3 Ca2 -164.02(15) 3_675 .
O4 Ca1 O3 Ca2 62.59(15) 3_675 .
O1 Ca1 O3 Ca2 -20.35(13) . .
O10 Ca1 O3 Ca2 -81.12(14) 1_565 .
Cl1A Ca1 O3 Ca2 -101.3(2) 3_675 .
Cl1B Ca1 O3 Ca2 0.5(2) 3_675 .
O9 Ca1 O3 Ca2 129.29(12) 3_675 .
P1 Ca1 O3 Ca2 -50.72(10) . .
Cl1B Ca1 O3 Ca2 12.4(2) 1_655 .
Cl1A Ca1 O3 Ca2 -113.81(15) 1_665 .
P2 Ca1 O3 Ca2 129.2(3) . .
O7 Ca2 O3 P2 87.09(16) . .
O9 Ca2 O3 P2 12.6(2) . .
O8 Ca2 O3 P2 151.45(18) . .
O2 Ca2 O3 P2 -144.93(18) . .
O5 Ca2 O3 P2 -66.43(16) . .
O6 Ca2 O3 P2 -94.82(18) . .
O4 Ca2 O3 P2 6.48(13) . .
O1 Ca2 O3 P2 156.65(19) . .
P1 Ca2 O3 P2 -172.55(18) . .
P3 Ca2 O3 P2 -82.04(15) . .
O7 Ca2 O3 Ca1 -50.49(14) . .
O9 Ca2 O3 Ca1 -124.97(13) . .
O8 Ca2 O3 Ca1 13.9(3) . .
O2 Ca2 O3 Ca1 77.49(13) . .
O5 Ca2 O3 Ca1 156.00(15) . .
O6 Ca2 O3 Ca1 127.61(13) . .
O4 Ca2 O3 Ca1 -131.10(18) . .
O1 Ca2 O3 Ca1 19.07(12) . .
P2 Ca2 O3 Ca1 -137.6(3) . .
P1 Ca2 O3 Ca1 49.87(10) . .
P3 Ca2 O3 Ca1 140.39(11) . .
O7 Ca2 O3 Ca3 -167.12(10) . 1_565
O9 Ca2 O3 Ca3 118.40(12) . 1_565
O8 Ca2 O3 Ca3 -102.8(2) . 1_565
O2 Ca2 O3 Ca3 -39.14(9) . 1_565
O5 Ca2 O3 Ca3 39.36(9) . 1_565
O6 Ca2 O3 Ca3 10.97(14) . 1_565
O4 Ca2 O3 Ca3 112.27(13) . 1_565
O1 Ca2 O3 Ca3 -97.57(11) . 1_565
P2 Ca2 O3 Ca3 105.79(17) . 1_565
P1 Ca2 O3 Ca3 -66.76(7) . 1_565
P3 Ca2 O3 Ca3 23.75(8) . 1_565
O7 Ca2 O4 P2 -101.50(15) . .
O9 Ca2 O4 P2 178.92(17) . .
O8 Ca2 O4 P2 -155.81(15) . .
O3 Ca2 O4 P2 -6.29(12) . .
O2 Ca2 O4 P2 27.84(19) . .
O5 Ca2 O4 P2 80.93(15) . .
O6 Ca2 O4 P2 108.64(15) . .
O1 Ca2 O4 P2 -37.49(17) . .
P1 Ca2 O4 P2 -5.25(18) . .
P3 Ca2 O4 P2 91.58(13) . .
O7 Ca2 O4 Ca1 39.35(12) . 3_675
O9 Ca2 O4 Ca1 -40.24(12) . 3_675
O8 Ca2 O4 Ca1 -15.0(2) . 3_675
O3 Ca2 O4 Ca1 134.55(17) . 3_675
O2 Ca2 O4 Ca1 168.69(10) . 3_675
O5 Ca2 O4 Ca1 -138.22(15) . 3_675
O6 Ca2 O4 Ca1 -110.51(12) . 3_675
O1 Ca2 O4 Ca1 103.36(13) . 3_675
P2 Ca2 O4 Ca1 140.8(2) . 3_675
P1 Ca2 O4 Ca1 135.60(8) . 3_675
P3 Ca2 O4 Ca1 -127.57(10) . 3_675
O7 Ca2 O4 Ca4 161.72(12) . 1_565
O9 Ca2 O4 Ca4 82.14(12) . 1_565
O8 Ca2 O4 Ca4 107.41(17) . 1_565
O3 Ca2 O4 Ca4 -103.07(14) . 1_565
O2 Ca2 O4 Ca4 -68.94(14) . 1_565
O5 Ca2 O4 Ca4 -15.85(10) . 1_565
O6 Ca2 O4 Ca4 11.86(14) . 1_565
O1 Ca2 O4 Ca4 -134.26(10) . 1_565
P2 Ca2 O4 Ca4 -96.78(16) . 1_565
P1 Ca2 O4 Ca4 -102.02(9) . 1_565
P3 Ca2 O4 Ca4 -5.20(9) . 1_565
O7 Ca2 O5 P3 151.76(18) . .
O9 Ca2 O5 P3 87.13(16) . .
O8 Ca2 O5 P3 12.6(2) . .
O3 Ca2 O5 P3 -145.00(17) . .
O2 Ca2 O5 P3 -66.43(16) . .
O6 Ca2 O5 P3 6.69(13) . .
O4 Ca2 O5 P3 156.58(19) . .
O1 Ca2 O5 P3 -94.94(18) . .
P2 Ca2 O5 P3 -172.55(18) . .
P1 Ca2 O5 P3 -82.01(15) . .
O7 Ca2 O5 Ca4 14.3(3) . 1_565
O9 Ca2 O5 Ca4 -50.37(14) . 1_565
O8 Ca2 O5 Ca4 -124.92(13) . 1_565
O3 Ca2 O5 Ca4 77.51(14) . 1_565
O2 Ca2 O5 Ca4 156.07(15) . 1_565
O6 Ca2 O5 Ca4 -130.81(18) . 1_565
O4 Ca2 O5 Ca4 19.08(12) . 1_565
O1 Ca2 O5 Ca4 127.56(14) . 1_565
P2 Ca2 O5 Ca4 49.95(10) . 1_565
P1 Ca2 O5 Ca4 140.50(11) . 1_565
P3 Ca2 O5 Ca4 -137.5(2) . 1_565
O7 Ca2 O5 Ca3 -102.6(2) . 1_565
O9 Ca2 O5 Ca3 -167.28(10) . 1_565
O8 Ca2 O5 Ca3 118.17(12) . 1_565
O3 Ca2 O5 Ca3 -39.40(9) . 1_565
O2 Ca2 O5 Ca3 39.16(9) . 1_565
O6 Ca2 O5 Ca3 112.28(13) . 1_565
O4 Ca2 O5 Ca3 -97.83(11) . 1_565
O1 Ca2 O5 Ca3 10.65(14) . 1_565
P2 Ca2 O5 Ca3 -66.96(7) . 1_565
P1 Ca2 O5 Ca3 23.59(8) . 1_565
P3 Ca2 O5 Ca3 105.59(17) . 1_565
O7 Ca2 O6 P3 -156.05(15) . .
O9 Ca2 O6 P3 -101.91(15) . .
O8 Ca2 O6 P3 178.48(17) . .
O3 Ca2 O6 P3 27.33(19) . .
O2 Ca2 O6 P3 80.56(15) . .
O5 Ca2 O6 P3 -6.52(12) . .
O4 Ca2 O6 P3 -37.94(17) . .
O1 Ca2 O6 P3 108.18(15) . .
P2 Ca2 O6 P3 -5.70(17) . .
P1 Ca2 O6 P3 91.25(13) . .
O7 Ca2 O6 Ca4 -14.7(2) . 2_655
O9 Ca2 O6 Ca4 39.46(12) . 2_655
O8 Ca2 O6 Ca4 -40.15(12) . 2_655
O3 Ca2 O6 Ca4 168.70(10) . 2_655
O2 Ca2 O6 Ca4 -138.08(15) . 2_655
O5 Ca2 O6 Ca4 134.85(16) . 2_655
O4 Ca2 O6 Ca4 103.43(13) . 2_655
O1 Ca2 O6 Ca4 -110.45(12) . 2_655
P2 Ca2 O6 Ca4 135.67(9) . 2_655
P1 Ca2 O6 Ca4 -127.38(10) . 2_655
P3 Ca2 O6 Ca4 141.4(2) . 2_655
O7 Ca2 O6 Ca5 107.44(17) . 2_655
O9 Ca2 O6 Ca5 161.58(12) . 2_655
O8 Ca2 O6 Ca5 81.97(12) . 2_655
O3 Ca2 O6 Ca5 -69.18(14) . 2_655
O2 Ca2 O6 Ca5 -15.96(10) . 2_655
O5 Ca2 O6 Ca5 -103.03(14) . 2_655
O4 Ca2 O6 Ca5 -134.45(10) . 2_655
O1 Ca2 O6 Ca5 11.67(14) . 2_655
P2 Ca2 O6 Ca5 -102.21(10) . 2_655
P1 Ca2 O6 Ca5 -5.26(9) . 2_655
P3 Ca2 O6 Ca5 -96.51(16) . 2_655
O9 Ca2 O7 P2 115.7(2) . 3_675
O8 Ca2 O7 P2 -164.5(2) . 3_675
O3 Ca2 O7 P2 -11.9(2) . 3_675
O2 Ca2 O7 P2 -83.8(2) . 3_675
O5 Ca2 O7 P2 48.0(4) . 3_675
O6 Ca2 O7 P2 170.92(18) . 3_675
O4 Ca2 O7 P2 43.5(2) . 3_675
O1 Ca2 O7 P2 -78.6(2) . 3_675
P2 Ca2 O7 P2 15.7(2) . 3_675
P1 Ca2 O7 P2 -78.0(2) . 3_675
P3 Ca2 O7 P2 116.1(3) . 3_675
O9 Ca2 O7 Ca3 -39.92(9) . .
O8 Ca2 O7 Ca3 39.94(9) . .
O3 Ca2 O7 Ca3 -167.46(10) . .
O2 Ca2 O7 Ca3 120.62(12) . .
O5 Ca2 O7 Ca3 -107.6(2) . .
O6 Ca2 O7 Ca3 15.3(2) . .
O4 Ca2 O7 Ca3 -112.09(10) . .
O1 Ca2 O7 Ca3 125.77(11) . .
P2 Ca2 O7 Ca3 -139.92(7) . .
P1 Ca2 O7 Ca3 126.39(7) . .
P3 Ca2 O7 Ca3 -39.5(4) . .
O9 Ca2 O7 Ca5 -136.04(11) . 1_655
O8 Ca2 O7 Ca5 -56.18(10) . 1_655
O3 Ca2 O7 Ca5 96.42(10) . 1_655
O2 Ca2 O7 Ca5 24.50(16) . 1_655
O5 Ca2 O7 Ca5 156.30(18) . 1_655
O6 Ca2 O7 Ca5 -80.79(19) . 1_655
O4 Ca2 O7 Ca5 151.79(11) . 1_655
O1 Ca2 O7 Ca5 29.65(9) . 1_655
P2 Ca2 O7 Ca5 123.96(8) . 1_655
P1 Ca2 O7 Ca5 30.27(9) . 1_655
P3 Ca2 O7 Ca5 -135.6(3) . 1_655
O9 Ca3 O7 P2 -116.3(2) . 3_675
O8 Ca3 O7 P2 164.4(2) . 3_675
O2 Ca3 O7 P2 84.8(2) 1_545 3_675
O5 Ca3 O7 P2 -51.0(4) 1_545 3_675
O3 Ca3 O7 P2 11.4(2) 1_545 3_675
O10 Ca3 O7 P2 78.7(2) . 3_675
O12 Ca3 O7 P2 -44.2(2) . 3_675
O11 Ca3 O7 P2 -170.73(18) . 3_675
P1 Ca3 O7 P2 78.2(2) 1_545 3_675
P3 Ca3 O7 P2 -119.4(3) 1_545 3_675
P2 Ca3 O7 P2 -16.3(2) 1_545 3_675
O9 Ca3 O7 Ca2 39.63(9) . .
O8 Ca3 O7 Ca2 -39.68(9) . .
O2 Ca3 O7 Ca2 -119.28(12) 1_545 .
O5 Ca3 O7 Ca2 104.8(2) 1_545 .
O3 Ca3 O7 Ca2 167.25(10) 1_545 .
O10 Ca3 O7 Ca2 -125.40(11) . .
O12 Ca3 O7 Ca2 111.68(10) . .
O11 Ca3 O7 Ca2 -14.8(2) . .
P1 Ca3 O7 Ca2 -125.87(7) 1_545 .
P3 Ca3 O7 Ca2 36.5(4) 1_545 .
P2 Ca3 O7 Ca2 139.59(7) 1_545 .
O9 Ca3 O7 Ca5 135.86(11) . 1_655
O8 Ca3 O7 Ca5 56.55(10) . 1_655
O2 Ca3 O7 Ca5 -23.05(16) 1_545 1_655
O5 Ca3 O7 Ca5 -158.92(18) 1_545 1_655
O3 Ca3 O7 Ca5 -96.52(10) 1_545 1_655
O10 Ca3 O7 Ca5 -29.17(9) . 1_655
O12 Ca3 O7 Ca5 -152.09(11) . 1_655
O11 Ca3 O7 Ca5 81.38(18) . 1_655
P1 Ca3 O7 Ca5 -29.64(9) 1_545 1_655
P3 Ca3 O7 Ca5 132.7(3) 1_545 1_655
P2 Ca3 O7 Ca5 -124.19(8) 1_545 1_655
O7 Ca2 O8 P1 116.0(2) . 2_745
O9 Ca2 O8 P1 -164.2(2) . 2_745
O3 Ca2 O8 P1 48.6(4) . 2_745
O2 Ca2 O8 P1 -11.6(2) . 2_745
O5 Ca2 O8 P1 -83.6(2) . 2_745
O6 Ca2 O8 P1 -78.4(2) . 2_745
O4 Ca2 O8 P1 171.42(18) . 2_745
O1 Ca2 O8 P1 43.8(2) . 2_745
P2 Ca2 O8 P1 116.5(3) . 2_745
P1 Ca2 O8 P1 16.0(2) . 2_745
P3 Ca2 O8 P1 -77.7(2) . 2_745
O7 Ca2 O8 Ca3 -39.99(9) . .
O9 Ca2 O8 Ca3 39.87(9) . .
O3 Ca2 O8 Ca3 -107.3(2) . .
O2 Ca2 O8 Ca3 -167.55(10) . .
O5 Ca2 O8 Ca3 120.49(12) . .
O6 Ca2 O8 Ca3 125.63(11) . .
O4 Ca2 O8 Ca3 15.5(2) . .
O1 Ca2 O8 Ca3 -112.20(10) . .
P2 Ca2 O8 Ca3 -39.4(4) . .
P1 Ca2 O8 Ca3 -139.97(7) . .
P3 Ca2 O8 Ca3 126.37(7) . .
O7 Ca2 O8 Ca4 -136.15(11) . 2_655
O9 Ca2 O8 Ca4 -56.29(10) . 2_655
O3 Ca2 O8 Ca4 156.50(18) . 2_655
O2 Ca2 O8 Ca4 96.29(10) . 2_655
O5 Ca2 O8 Ca4 24.33(16) . 2_655
O6 Ca2 O8 Ca4 29.47(9) . 2_655
O4 Ca2 O8 Ca4 -80.70(19) . 2_655
O1 Ca2 O8 Ca4 151.64(11) . 2_655
P2 Ca2 O8 Ca4 -135.6(3) . 2_655
P1 Ca2 O8 Ca4 123.87(8) . 2_655
P3 Ca2 O8 Ca4 30.21(9) . 2_655
O9 Ca3 O8 P1 164.4(2) . 2_745
O7 Ca3 O8 P1 -116.4(2) . 2_745
O2 Ca3 O8 P1 11.4(2) 1_545 2_745
O5 Ca3 O8 P1 84.8(2) 1_545 2_745
O3 Ca3 O8 P1 -51.1(4) 1_545 2_745
O10 Ca3 O8 P1 -44.4(2) . 2_745
O12 Ca3 O8 P1 -170.85(18) . 2_745
O11 Ca3 O8 P1 78.6(2) . 2_745
P1 Ca3 O8 P1 -16.4(2) 1_545 2_745
P3 Ca3 O8 P1 78.2(2) 1_545 2_745
P2 Ca3 O8 P1 -119.3(3) 1_545 2_745
O9 Ca3 O8 Ca2 -39.55(9) . .
O7 Ca3 O8 Ca2 39.61(9) . .
O2 Ca3 O8 Ca2 167.38(10) 1_545 .
O5 Ca3 O8 Ca2 -119.22(12) 1_545 .
O3 Ca3 O8 Ca2 105.0(2) 1_545 .
O10 Ca3 O8 Ca2 111.67(10) . .
O12 Ca3 O8 Ca2 -14.8(2) . .
O11 Ca3 O8 Ca2 -125.33(11) . .
P1 Ca3 O8 Ca2 139.62(7) 1_545 .
P3 Ca3 O8 Ca2 -125.81(7) 1_545 .
P2 Ca3 O8 Ca2 36.7(3) 1_545 .
O9 Ca3 O8 Ca4 56.56(10) . 2_655
O7 Ca3 O8 Ca4 135.72(11) . 2_655
O2 Ca3 O8 Ca4 -96.51(10) 1_545 2_655
O5 Ca3 O8 Ca4 -23.11(16) 1_545 2_655
O3 Ca3 O8 Ca4 -158.92(18) 1_545 2_655
O10 Ca3 O8 Ca4 -152.22(11) . 2_655
O12 Ca3 O8 Ca4 81.29(18) . 2_655
O11 Ca3 O8 Ca4 -29.22(9) . 2_655
P1 Ca3 O8 Ca4 -124.27(8) 1_545 2_655
P3 Ca3 O8 Ca4 -29.70(9) 1_545 2_655
P2 Ca3 O8 Ca4 132.8(3) 1_545 2_655
O7 Ca2 O9 P3 -164.2(2) . 2_645
O8 Ca2 O9 P3 115.9(2) . 2_645
O3 Ca2 O9 P3 -83.7(2) . 2_645
O2 Ca2 O9 P3 48.3(4) . 2_645
O5 Ca2 O9 P3 -11.7(2) . 2_645
O6 Ca2 O9 P3 43.7(2) . 2_645
O4 Ca2 O9 P3 -78.4(2) . 2_645
O1 Ca2 O9 P3 171.30(18) . 2_645
P2 Ca2 O9 P3 -77.8(2) . 2_645
P1 Ca2 O9 P3 116.6(3) . 2_645
P3 Ca2 O9 P3 15.9(2) . 2_645
O7 Ca2 O9 Ca3 39.99(9) . .
O8 Ca2 O9 Ca3 -39.88(9) . .
O3 Ca2 O9 Ca3 120.49(12) . .
O2 Ca2 O9 Ca3 -107.5(2) . .
O5 Ca2 O9 Ca3 -167.52(10) . .
O6 Ca2 O9 Ca3 -112.12(10) . .
O4 Ca2 O9 Ca3 125.85(11) . .
O1 Ca2 O9 Ca3 15.5(2) . .
P2 Ca2 O9 Ca3 126.37(7) . .
P1 Ca2 O9 Ca3 -39.2(4) . .
P3 Ca2 O9 Ca3 -139.91(7) . .
O7 Ca2 O9 Ca1 -56.22(10) . 3_675
O8 Ca2 O9 Ca1 -136.09(11) . 3_675
O3 Ca2 O9 Ca1 24.28(16) . 3_675
O2 Ca2 O9 Ca1 156.27(18) . 3_675
O5 Ca2 O9 Ca1 96.26(10) . 3_675
O6 Ca2 O9 Ca1 151.67(11) . 3_675
O4 Ca2 O9 Ca1 29.64(9) . 3_675
O1 Ca2 O9 Ca1 -80.7(2) . 3_675
P2 Ca2 O9 Ca1 30.16(9) . 3_675
P1 Ca2 O9 Ca1 -135.4(3) . 3_675
P3 Ca2 O9 Ca1 123.88(8) . 3_675
O8 Ca3 O9 P3 -116.3(2) . 2_645
O7 Ca3 O9 P3 164.5(2) . 2_645
O2 Ca3 O9 P3 -50.9(4) 1_545 2_645
O5 Ca3 O9 P3 11.5(2) 1_545 2_645
O3 Ca3 O9 P3 84.8(2) 1_545 2_645
O10 Ca3 O9 P3 -170.83(19) . 2_645
O12 Ca3 O9 P3 78.7(2) . 2_645
O11 Ca3 O9 P3 -44.2(2) . 2_645
P1 Ca3 O9 P3 -119.5(3) 1_545 2_645
P3 Ca3 O9 P3 -16.3(2) 1_545 2_645
P2 Ca3 O9 P3 78.2(2) 1_545 2_645
O8 Ca3 O9 Ca2 39.60(9) . .
O7 Ca3 O9 Ca2 -39.61(9) . .
O2 Ca3 O9 Ca2 104.9(2) 1_545 .
O5 Ca3 O9 Ca2 167.38(10) 1_545 .
O3 Ca3 O9 Ca2 -119.34(12) 1_545 .
O10 Ca3 O9 Ca2 -15.0(2) . .
O12 Ca3 O9 Ca2 -125.41(11) . .
O11 Ca3 O9 Ca2 111.67(10) . .
P1 Ca3 O9 Ca2 36.4(4) 1_545 .
P3 Ca3 O9 Ca2 139.59(7) 1_545 .
P2 Ca3 O9 Ca2 -125.89(7) 1_545 .
O8 Ca3 O9 Ca1 135.87(11) . 3_675
O7 Ca3 O9 Ca1 56.65(10) . 3_675
O2 Ca3 O9 Ca1 -158.80(18) 1_545 3_675
O5 Ca3 O9 Ca1 -96.35(10) 1_545 3_675
O3 Ca3 O9 Ca1 -23.08(16) 1_545 3_675
O10 Ca3 O9 Ca1 81.31(19) . 3_675
O12 Ca3 O9 Ca1 -29.15(9) . 3_675
O11 Ca3 O9 Ca1 -152.06(11) . 3_675
P1 Ca3 O9 Ca1 132.6(3) 1_545 3_675
P3 Ca3 O9 Ca1 -124.15(8) 1_545 3_675
P2 Ca3 O9 Ca1 -29.62(9) 1_545 3_675
O9 Ca3 O10 P1 155.51(15) . 1_545
O8 Ca3 O10 P1 102.24(16) . 1_545
O7 Ca3 O10 P1 -179.02(18) . 1_545
O2 Ca3 O10 P1 6.90(13) 1_545 1_545
O5 Ca3 O10 P1 -27.4(2) 1_545 1_545
O3 Ca3 O10 P1 -81.34(15) 1_545 1_545
O12 Ca3 O10 P1 -109.65(15) . 1_545
O11 Ca3 O10 P1 39.05(18) . 1_545
P3 Ca3 O10 P1 6.44(18) 1_545 1_545
P2 Ca3 O10 P1 -92.03(14) 1_545 1_545
O9 Ca3 O10 Ca5 14.3(3) . 1_655
O8 Ca3 O10 Ca5 -38.93(13) . 1_655
O7 Ca3 O10 Ca5 39.81(12) . 1_655
O2 Ca3 O10 Ca5 -134.27(18) 1_545 1_655
O5 Ca3 O10 Ca5 -168.55(11) 1_545 1_655
O3 Ca3 O10 Ca5 137.49(16) 1_545 1_655
O12 Ca3 O10 Ca5 109.18(13) . 1_655
O11 Ca3 O10 Ca5 -102.13(13) . 1_655
P1 Ca3 O10 Ca5 -141.2(2) 1_545 1_655
P3 Ca3 O10 Ca5 -134.74(9) 1_545 1_655
P2 Ca3 O10 Ca5 126.80(11) 1_545 1_655
O9 Ca3 O10 Ca1 -107.95(17) . 1_545
O8 Ca3 O10 Ca1 -161.22(12) . 1_545
O7 Ca3 O10 Ca1 -82.48(12) . 1_545
O2 Ca3 O10 Ca1 103.44(14) 1_545 1_545
O5 Ca3 O10 Ca1 69.16(15) 1_545 1_545
O3 Ca3 O10 Ca1 15.20(10) 1_545 1_545
O12 Ca3 O10 Ca1 -13.12(14) . 1_545
O11 Ca3 O10 Ca1 135.58(10) . 1_545
P1 Ca3 O10 Ca1 96.53(16) 1_545 1_545
P3 Ca3 O10 Ca1 102.97(10) 1_545 1_545
P2 Ca3 O10 Ca1 4.51(9) 1_545 1_545
O9 Ca3 O11 P3 102.19(15) . 1_545
O8 Ca3 O11 P3 -179.02(17) . 1_545
O7 Ca3 O11 P3 155.33(15) . 1_545
O2 Ca3 O11 P3 -81.42(15) 1_545 1_545
O5 Ca3 O11 P3 6.90(12) 1_545 1_545
O3 Ca3 O11 P3 -27.26(19) 1_545 1_545
O10 Ca3 O11 P3 -109.74(15) . 1_545
O12 Ca3 O11 P3 38.96(17) . 1_545
P1 Ca3 O11 P3 -92.11(13) 1_545 1_545
P2 Ca3 O11 P3 6.36(17) 1_545 1_545
O9 Ca3 O11 Ca4 -38.94(12) . 2_655
O8 Ca3 O11 Ca4 39.85(12) . 2_655
O7 Ca3 O11 Ca4 14.2(2) . 2_655
O2 Ca3 O11 Ca4 137.46(15) 1_545 2_655
O5 Ca3 O11 Ca4 -134.23(16) 1_545 2_655
O3 Ca3 O11 Ca4 -168.38(10) 1_545 2_655
O10 Ca3 O11 Ca4 109.14(12) . 2_655
O12 Ca3 O11 Ca4 -102.16(13) . 2_655
P1 Ca3 O11 Ca4 126.77(10) 1_545 2_655
P3 Ca3 O11 Ca4 -141.1(2) 1_545 2_655
P2 Ca3 O11 Ca4 -134.77(9) 1_545 2_655
O9 Ca3 O11 Ca5 -161.16(12) . 2_645
O8 Ca3 O11 Ca5 -82.37(12) . 2_645
O7 Ca3 O11 Ca5 -108.02(17) . 2_645
O2 Ca3 O11 Ca5 15.23(10) 1_545 2_645
O5 Ca3 O11 Ca5 103.55(14) 1_545 2_645
O3 Ca3 O11 Ca5 69.39(14) 1_545 2_645
O10 Ca3 O11 Ca5 -13.09(14) . 2_645
O12 Ca3 O11 Ca5 135.61(10) . 2_645
P1 Ca3 O11 Ca5 4.54(9) 1_545 2_645
P3 Ca3 O11 Ca5 96.65(16) 1_545 2_645
P2 Ca3 O11 Ca5 103.01(10) 1_545 2_645
O5 Ca4 O12 P2 75.96(17) 1_545 1_545
O6 Ca4 O12 P2 165.01(18) 2_645 1_545
O11 Ca4 O12 P2 8.6(3) 2_645 1_545
O4 Ca4 O12 P2 -5.65(11) 1_545 1_545
Cl1B Ca4 O12 P2 -66.92(16) 3_565 1_545
Cl1A Ca4 O12 P2 -116.41(17) 3_565 1_545
O8 Ca4 O12 P2 169.47(13) 2_645 1_545
Cl1B Ca4 O12 P2 -57.37(16) 1_545 1_545
Cl1A Ca4 O12 P2 -129.81(18) . 1_545
P3 Ca4 O12 P2 87.14(15) 1_545 1_545
O5 Ca4 O12 Ca1 -125.33(18) 1_545 3_675
O6 Ca4 O12 Ca1 -36.27(16) 2_645 3_675
O11 Ca4 O12 Ca1 167.36(15) 2_645 3_675
O4 Ca4 O12 Ca1 153.1(2) 1_545 3_675
Cl1B Ca4 O12 Ca1 91.79(16) 3_565 3_675
Cl1A Ca4 O12 Ca1 42.31(14) 3_565 3_675
O8 Ca4 O12 Ca1 -31.8(3) 2_645 3_675
P2 Ca4 O12 Ca1 158.7(3) 1_545 3_675
Cl1B Ca4 O12 Ca1 101.34(15) 1_545 3_675
Cl1A Ca4 O12 Ca1 28.91(13) . 3_675
P3 Ca4 O12 Ca1 -114.15(15) 1_545 3_675
O5 Ca4 O12 Ca3 -15.44(11) 1_545 .
O6 Ca4 O12 Ca3 73.62(12) 2_645 .
O11 Ca4 O12 Ca3 -82.75(19) 2_645 .
O4 Ca4 O12 Ca3 -97.05(15) 1_545 .
Cl1B Ca4 O12 Ca3 -158.32(9) 3_565 .
Cl1A Ca4 O12 Ca3 152.19(11) 3_565 .
O8 Ca4 O12 Ca3 78.1(2) 2_645 .
P2 Ca4 O12 Ca3 -91.40(16) 1_545 .
Cl1B Ca4 O12 Ca3 -148.77(8) 1_545 .
Cl1A Ca4 O12 Ca3 138.79(12) . .
P3 Ca4 O12 Ca3 -4.26(9) 1_545 .
O9 Ca3 O12 P2 -179.02(17) . 1_545
O8 Ca3 O12 P2 155.41(15) . 1_545
O7 Ca3 O12 P2 102.30(15) . 1_545
O2 Ca3 O12 P2 -27.3(2) 1_545 1_545
O5 Ca3 O12 P2 -81.36(15) 1_545 1_545
O3 Ca3 O12 P2 6.87(12) 1_545 1_545
O10 Ca3 O12 P2 39.08(17) . 1_545
O11 Ca3 O12 P2 -109.63(15) . 1_545
P1 Ca3 O12 P2 6.44(18) 1_545 1_545
P3 Ca3 O12 P2 -92.06(13) 1_545 1_545
O9 Ca3 O12 Ca1 39.80(12) . 3_675
O8 Ca3 O12 Ca1 14.2(2) . 3_675
O7 Ca3 O12 Ca1 -38.87(13) . 3_675
O2 Ca3 O12 Ca1 -168.48(10) 1_545 3_675
O5 Ca3 O12 Ca1 137.46(15) 1_545 3_675
O3 Ca3 O12 Ca1 -134.30(17) 1_545 3_675
O10 Ca3 O12 Ca1 -102.09(13) . 3_675
O11 Ca3 O12 Ca1 109.19(12) . 3_675
P1 Ca3 O12 Ca1 -134.74(9) 1_545 3_675
P3 Ca3 O12 Ca1 126.76(10) 1_545 3_675
P2 Ca3 O12 Ca1 -141.2(2) 1_545 3_675
O9 Ca3 O12 Ca4 -82.45(11) . .
O8 Ca3 O12 Ca4 -108.01(17) . .
O7 Ca3 O12 Ca4 -161.13(12) . .
O2 Ca3 O12 Ca4 69.27(14) 1_545 .
O5 Ca3 O12 Ca4 15.21(10) 1_545 .
O3 Ca3 O12 Ca4 103.45(14) 1_545 .
O10 Ca3 O12 Ca4 135.66(10) . .
O11 Ca3 O12 Ca4 -13.06(14) . .
P1 Ca3 O12 Ca4 103.01(9) 1_545 .
P3 Ca3 O12 Ca4 4.51(9) 1_545 .
P2 Ca3 O12 Ca4 96.57(16) 1_545 .
Ca5 O1 P1 O10 143.2(3) 1_655 1_565
Ca1 O1 P1 O10 -8.61(15) . 1_565
Ca2 O1 P1 O10 -105.63(15) . 1_565
Ca5 O1 P1 O8 19.4(3) 1_655 2_755
Ca1 O1 P1 O8 -132.37(15) . 2_755
Ca2 O1 P1 O8 130.60(14) . 2_755
Ca5 O1 P1 O2 -102.5(3) 1_655 .
Ca1 O1 P1 O2 105.65(15) . .
Ca2 O1 P1 O2 8.62(17) . .
Ca5 O1 P1 Ca1 151.8(3) 1_655 .
Ca2 O1 P1 Ca1 -97.03(12) . .
Ca5 O1 P1 Ca3 -152.0(2) 1_655 1_565
Ca1 O1 P1 Ca3 56.17(13) . 1_565
Ca2 O1 P1 Ca3 -40.86(12) . 1_565
Ca5 O1 P1 Ca2 -111.2(3) 1_655 .
Ca1 O1 P1 Ca2 97.03(12) . .
Ca5 O1 P1 Ca5 -67.9(3) 1_655 2_655
Ca1 O1 P1 Ca5 140.31(7) . 2_655
Ca2 O1 P1 Ca5 43.29(15) . 2_655
Ca5 O1 P1 Ca4 66.8(3) 1_655 1_665
Ca1 O1 P1 Ca4 -85.05(9) . 1_665
Ca2 O1 P1 Ca4 177.92(10) . 1_665
Ca5 O2 P1 O10 -122.8(2) 2_655 1_565
Ca3 O2 P1 O10 11.2(2) 1_565 1_565
Ca2 O2 P1 O10 104.60(19) . 1_565
Ca5 O2 P1 O1 122.4(2) 2_655 .
Ca3 O2 P1 O1 -103.58(19) 1_565 .
Ca2 O2 P1 O1 -10.2(2) . .
Ca5 O2 P1 O8 -0.1(3) 2_655 2_755
Ca3 O2 P1 O8 133.92(18) 1_565 2_755
Ca2 O2 P1 O8 -132.72(18) . 2_755
Ca5 O2 P1 Ca1 179.79(14) 2_655 .
Ca3 O2 P1 Ca1 -46.18(17) 1_565 .
Ca2 O2 P1 Ca1 47.18(17) . .
Ca5 O2 P1 Ca3 -134.0(3) 2_655 1_565
Ca2 O2 P1 Ca3 93.36(14) . 1_565
Ca5 O2 P1 Ca2 132.6(3) 2_655 .
Ca3 O2 P1 Ca2 -93.36(14) 1_565 .
Ca3 O2 P1 Ca5 134.0(3) 1_565 2_655
Ca2 O2 P1 Ca5 -132.6(3) . 2_655
Ca5 O2 P1 Ca4 -0.8(9) 2_655 1_665
Ca3 O2 P1 Ca4 133.2(6) 1_565 1_665
Ca2 O2 P1 Ca4 -133.4(6) . 1_665
O3 Ca1 P1 O10 -95.00(18) . 1_565
O12 Ca1 P1 O10 -15.92(18) 3_675 1_565
O4 Ca1 P1 O10 -174.19(18) 3_675 1_565
O1 Ca1 P1 O10 169.85(18) . 1_565
Cl1A Ca1 P1 O10 57.65(16) 3_675 1_565
Cl1B Ca1 P1 O10 112.95(16) 3_675 1_565
Cl1B Ca1 P1 O10 125.04(16) 1_655 1_565
Cl1A Ca1 P1 O10 44.88(16) 1_665 1_565
P2 Ca1 P1 O10 -95.04(16) . 1_565
O3 Ca1 P1 O1 95.14(18) . .
O12 Ca1 P1 O1 174.22(18) 3_675 .
O4 Ca1 P1 O1 15.96(18) 3_675 .
O10 Ca1 P1 O1 -169.85(18) 1_565 .
Cl1A Ca1 P1 O1 -112.21(16) 3_675 .
Cl1B Ca1 P1 O1 -56.91(16) 3_675 .
Cl1B Ca1 P1 O1 -44.81(16) 1_655 .
Cl1A Ca1 P1 O1 -124.97(16) 1_665 .
P2 Ca1 P1 O1 95.11(16) . .
O3 Ca1 P1 O8 179.7(2) . 2_755
O12 Ca1 P1 O8 -101.2(2) 3_675 2_755
O4 Ca1 P1 O8 100.5(2) 3_675 2_755
O1 Ca1 P1 O8 84.6(3) . 2_755
O10 Ca1 P1 O8 -85.3(3) 1_565 2_755
Cl1A Ca1 P1 O8 -27.7(2) 3_675 2_755
Cl1B Ca1 P1 O8 27.6(2) 3_675 2_755
Cl1B Ca1 P1 O8 39.7(2) 1_655 2_755
Cl1A Ca1 P1 O8 -40.4(2) 1_665 2_755
P2 Ca1 P1 O8 179.7(2) . 2_755
O3 Ca1 P1 O2 -0.16(19) . .
O12 Ca1 P1 O2 78.92(18) 3_675 .
O4 Ca1 P1 O2 -79.35(18) 3_675 .
O1 Ca1 P1 O2 -95.3(2) . .
O10 Ca1 P1 O2 94.8(2) 1_565 .
Cl1A Ca1 P1 O2 152.49(17) 3_675 .
Cl1B Ca1 P1 O2 -152.21(17) 3_675 .
Cl1B Ca1 P1 O2 -140.11(17) 1_655 .
Cl1A Ca1 P1 O2 139.73(17) 1_665 .
P2 Ca1 P1 O2 -0.19(16) . .
O3 Ca1 P1 Ca3 -32.63(10) . 1_565
O12 Ca1 P1 Ca3 46.45(9) 3_675 1_565
O4 Ca1 P1 Ca3 -111.82(9) 3_675 1_565
O1 Ca1 P1 Ca3 -127.78(16) . 1_565
O10 Ca1 P1 Ca3 62.37(15) 1_565 1_565
Cl1A Ca1 P1 Ca3 120.01(6) 3_675 1_565
Cl1B Ca1 P1 Ca3 175.31(6) 3_675 1_565
Cl1B Ca1 P1 Ca3 -172.59(5) 1_655 1_565
Cl1A Ca1 P1 Ca3 107.25(5) 1_665 1_565
P2 Ca1 P1 Ca3 -32.67(4) . 1_565
O3 Ca1 P1 Ca2 33.27(10) . .
O12 Ca1 P1 Ca2 112.35(9) 3_675 .
O4 Ca1 P1 Ca2 -45.91(9) 3_675 .
O1 Ca1 P1 Ca2 -61.87(15) . .
O10 Ca1 P1 Ca2 128.28(16) 1_565 .
Cl1A Ca1 P1 Ca2 -174.08(6) 3_675 .
Cl1B Ca1 P1 Ca2 -118.78(6) 3_675 .
Cl1B Ca1 P1 Ca2 -106.68(5) 1_655 .
Cl1A Ca1 P1 Ca2 173.16(5) 1_665 .
P2 Ca1 P1 Ca2 33.24(4) . .
O3 Ca1 P1 Ca5 0.06(13) . 2_655
O12 Ca1 P1 Ca5 79.14(13) 3_675 2_655
O4 Ca1 P1 Ca5 -79.13(13) 3_675 2_655
O1 Ca1 P1 Ca5 -95.08(18) . 2_655
O10 Ca1 P1 Ca5 95.06(18) 1_565 2_655
Cl1A Ca1 P1 Ca5 152.71(10) 3_675 2_655
Cl1B Ca1 P1 Ca5 -151.99(10) 3_675 2_655
Cl1B Ca1 P1 Ca5 -139.89(10) 1_655 2_655
Cl1A Ca1 P1 Ca5 139.95(10) 1_665 2_655
P2 Ca1 P1 Ca5 0.03(10) . 2_655
O3 Ca1 P1 Ca4 179.97(10) . 1_665
O12 Ca1 P1 Ca4 -100.95(9) 3_675 1_665
O4 Ca1 P1 Ca4 100.78(9) 3_675 1_665
O1 Ca1 P1 Ca4 84.83(16) . 1_665
O10 Ca1 P1 Ca4 -85.03(16) 1_565 1_665
Cl1A Ca1 P1 Ca4 -27.38(6) 3_675 1_665
Cl1B Ca1 P1 Ca4 27.92(6) 3_675 1_665
Cl1B Ca1 P1 Ca4 40.02(5) 1_655 1_665
Cl1A Ca1 P1 Ca4 -40.14(5) 1_665 1_665
P2 Ca1 P1 Ca4 179.94(4) . 1_665
O7 Ca2 P1 O10 97.12(16) . 1_565
O9 Ca2 P1 O10 173.7(4) . 1_565
O8 Ca2 P1 O10 174.37(16) . 1_565
O3 Ca2 P1 O10 11.42(16) . 1_565
O2 Ca2 P1 O10 -92.9(2) . 1_565
O5 Ca2 P1 O10 -58.78(16) . 1_565
O6 Ca2 P1 O10 -114.71(16) . 1_565
O4 Ca2 P1 O10 10.47(17) . 1_565
O1 Ca2 P1 O10 98.34(18) . 1_565
P2 Ca2 P1 O10 7.97(15) . 1_565
P3 Ca2 P1 O10 -86.20(15) . 1_565
O7 Ca2 P1 O1 -1.22(17) . .
O9 Ca2 P1 O1 75.4(4) . .
O8 Ca2 P1 O1 76.03(17) . .
O3 Ca2 P1 O1 -86.92(17) . .
O2 Ca2 P1 O1 168.8(2) . .
O5 Ca2 P1 O1 -157.12(17) . .
O6 Ca2 P1 O1 146.95(17) . .
O4 Ca2 P1 O1 -87.86(17) . .
P2 Ca2 P1 O1 -90.37(15) . .
P3 Ca2 P1 O1 175.46(15) . .
O7 Ca2 P1 O8 -93.4(2) . 2_755
O9 Ca2 P1 O8 -16.9(4) . 2_755
O8 Ca2 P1 O8 -16.2(2) . 2_755
O3 Ca2 P1 O8 -179.1(2) . 2_755
O2 Ca2 P1 O8 76.5(2) . 2_755
O5 Ca2 P1 O8 110.7(2) . 2_755
O6 Ca2 P1 O8 54.7(2) . 2_755
O4 Ca2 P1 O8 179.92(19) . 2_755
O1 Ca2 P1 O8 -92.2(2) . 2_755
P2 Ca2 P1 O8 177.42(18) . 2_755
P3 Ca2 P1 O8 83.25(18) . 2_755
O7 Ca2 P1 O2 -169.98(18) . .
O9 Ca2 P1 O2 -93.4(4) . .
O8 Ca2 P1 O2 -92.72(18) . .
O3 Ca2 P1 O2 104.32(18) . .
O5 Ca2 P1 O2 34.13(18) . .
O6 Ca2 P1 O2 -21.81(18) . .
O4 Ca2 P1 O2 103.38(19) . .
O1 Ca2 P1 O2 -168.8(2) . .
P2 Ca2 P1 O2 100.87(17) . .
P3 Ca2 P1 O2 6.70(17) . .
O7 Ca2 P1 Ca1 53.87(8) . .
O9 Ca2 P1 Ca1 130.4(3) . .
O8 Ca2 P1 Ca1 131.12(8) . .
O3 Ca2 P1 Ca1 -31.83(8) . .
O2 Ca2 P1 Ca1 -136.15(17) . .
O5 Ca2 P1 Ca1 -102.03(7) . .
O6 Ca2 P1 Ca1 -157.96(7) . .
O4 Ca2 P1 Ca1 -32.78(9) . .
O1 Ca2 P1 Ca1 55.09(15) . .
P2 Ca2 P1 Ca1 -35.28(3) . .
P3 Ca2 P1 Ca1 -129.45(4) . .
O7 Ca2 P1 Ca3 136.27(9) . 1_565
O9 Ca2 P1 Ca3 -147.2(3) . 1_565
O8 Ca2 P1 Ca3 -146.48(8) . 1_565
O3 Ca2 P1 Ca3 50.56(8) . 1_565
O2 Ca2 P1 Ca3 -53.76(16) . 1_565
O5 Ca2 P1 Ca3 -19.63(7) . 1_565
O6 Ca2 P1 Ca3 -75.56(7) . 1_565
O4 Ca2 P1 Ca3 49.62(9) . 1_565
O1 Ca2 P1 Ca3 137.48(16) . 1_565
P2 Ca2 P1 Ca3 47.12(3) . 1_565
P3 Ca2 P1 Ca3 -47.05(3) . 1_565
O7 Ca2 P1 Ca5 -144.12(8) . 2_655
O9 Ca2 P1 Ca5 -67.5(3) . 2_655
O8 Ca2 P1 Ca5 -66.87(8) . 2_655
O3 Ca2 P1 Ca5 130.17(9) . 2_655
O2 Ca2 P1 Ca5 25.85(16) . 2_655
O5 Ca2 P1 Ca5 59.98(7) . 2_655
O6 Ca2 P1 Ca5 4.05(7) . 2_655
O4 Ca2 P1 Ca5 129.23(9) . 2_655
O1 Ca2 P1 Ca5 -142.91(16) . 2_655
P2 Ca2 P1 Ca5 126.73(3) . 2_655
P3 Ca2 P1 Ca5 32.56(3) . 2_655
O7 Ca2 P1 Ca4 -4.43(10) . 1_665
O9 Ca2 P1 Ca4 72.1(4) . 1_665
O8 Ca2 P1 Ca4 72.82(10) . 1_665
O3 Ca2 P1 Ca4 -90.14(10) . 1_665
O2 Ca2 P1 Ca4 165.54(18) . 1_665
O5 Ca2 P1 Ca4 -160.33(9) . 1_665
O6 Ca2 P1 Ca4 143.73(9) . 1_665
O4 Ca2 P1 Ca4 -91.08(10) . 1_665
O1 Ca2 P1 Ca4 -3.22(15) . 1_665
P2 Ca2 P1 Ca4 -93.58(6) . 1_665
P3 Ca2 P1 Ca4 172.25(6) . 1_665
Ca1 O4 P2 O12 143.0(3) 3_675 1_565
Ca4 O4 P2 O12 -8.35(16) 1_565 1_565
Ca2 O4 P2 O12 -105.54(16) . 1_565
Ca1 O4 P2 O7 19.3(3) 3_675 3_675
Ca4 O4 P2 O7 -132.02(15) 1_565 3_675
Ca2 O4 P2 O7 130.80(14) . 3_675
Ca1 O4 P2 O3 -102.8(3) 3_675 .
Ca4 O4 P2 O3 105.83(16) 1_565 .
Ca2 O4 P2 O3 8.65(17) . .
Ca1 O4 P2 Ca4 151.4(4) 3_675 1_565
Ca2 O4 P2 Ca4 -97.19(13) . 1_565
Ca1 O4 P2 Ca3 -152.3(2) 3_675 1_565
Ca4 O4 P2 Ca3 56.33(13) 1_565 1_565
Ca2 O4 P2 Ca3 -40.86(12) . 1_565
Ca1 O4 P2 Ca2 -111.5(3) 3_675 .
Ca4 O4 P2 Ca2 97.19(13) 1_565 .
Ca1 O4 P2 Ca1 -68.4(3) 3_675 .
Ca4 O4 P2 Ca1 140.27(7) 1_565 .
Ca2 O4 P2 Ca1 43.08(15) . .
Ca1 O4 P2 Ca5 66.5(3) 3_675 3_575
Ca4 O4 P2 Ca5 -84.88(10) 1_565 3_575
Ca2 O4 P2 Ca5 177.93(9) . 3_575
Ca1 O3 P2 O12 -122.6(2) . 1_565
Ca3 O3 P2 O12 11.2(2) 1_565 1_565
Ca2 O3 P2 O12 104.46(18) . 1_565
Ca1 O3 P2 O4 122.7(2) . .
Ca3 O3 P2 O4 -103.49(18) 1_565 .
Ca2 O3 P2 O4 -10.2(2) . .
Ca1 O3 P2 O7 -0.1(3) . 3_675
Ca3 O3 P2 O7 133.74(17) 1_565 3_675
Ca2 O3 P2 O7 -133.00(17) . 3_675
Ca1 O3 P2 Ca4 -179.98(14) . 1_565
Ca3 O3 P2 Ca4 -46.19(17) 1_565 1_565
Ca2 O3 P2 Ca4 47.07(17) . 1_565
Ca1 O3 P2 Ca3 -133.8(3) . 1_565
Ca2 O3 P2 Ca3 93.26(14) . 1_565
Ca1 O3 P2 Ca2 132.9(3) . .
Ca3 O3 P2 Ca2 -93.26(14) 1_565 .
Ca3 O3 P2 Ca1 133.8(3) 1_565 .
Ca2 O3 P2 Ca1 -132.9(3) . .
Ca1 O3 P2 Ca5 -0.4(9) . 3_575
Ca3 O3 P2 Ca5 133.4(6) 1_565 3_575
Ca2 O3 P2 Ca5 -133.3(6) . 3_575
O7 Ca2 P2 O12 174.48(16) . 1_565
O9 Ca2 P2 O12 97.25(16) . 1_565
O8 Ca2 P2 O12 173.9(3) . 1_565
O3 Ca2 P2 O12 -93.0(2) . 1_565
O2 Ca2 P2 O12 -58.75(16) . 1_565
O5 Ca2 P2 O12 11.43(16) . 1_565
O6 Ca2 P2 O12 10.69(17) . 1_565
O4 Ca2 P2 O12 98.29(18) . 1_565
O1 Ca2 P2 O12 -114.62(15) . 1_565
P1 Ca2 P2 O12 -86.16(14) . 1_565
P3 Ca2 P2 O12 7.97(14) . 1_565
O7 Ca2 P2 O4 76.20(16) . .
O9 Ca2 P2 O4 -1.04(17) . .
O8 Ca2 P2 O4 75.6(4) . .
O3 Ca2 P2 O4 168.7(2) . .
O2 Ca2 P2 O4 -157.04(16) . .
O5 Ca2 P2 O4 -86.86(17) . .
O6 Ca2 P2 O4 -87.60(17) . .
O1 Ca2 P2 O4 147.09(16) . .
P1 Ca2 P2 O4 175.55(15) . .
P3 Ca2 P2 O4 -90.32(15) . .
O7 Ca2 P2 O7 -16.1(2) . 3_675
O9 Ca2 P2 O7 -93.4(2) . 3_675
O8 Ca2 P2 O7 -16.7(4) . 3_675
O3 Ca2 P2 O7 76.4(2) . 3_675
O2 Ca2 P2 O7 110.63(19) . 3_675
O5 Ca2 P2 O7 -179.2(2) . 3_675
O6 Ca2 P2 O7 -179.93(19) . 3_675
O4 Ca2 P2 O7 -92.3(2) . 3_675
O1 Ca2 P2 O7 54.8(2) . 3_675
P1 Ca2 P2 O7 83.22(18) . 3_675
P3 Ca2 P2 O7 177.35(18) . 3_675
O7 Ca2 P2 O3 -92.51(18) . .
O9 Ca2 P2 O3 -169.75(18) . .
O8 Ca2 P2 O3 -93.1(4) . .
O2 Ca2 P2 O3 34.25(18) . .
O5 Ca2 P2 O3 104.43(18) . .
O6 Ca2 P2 O3 103.69(18) . .
O4 Ca2 P2 O3 -168.7(2) . .
O1 Ca2 P2 O3 -21.62(18) . .
P1 Ca2 P2 O3 6.84(16) . .
P3 Ca2 P2 O3 100.97(17) . .
O7 Ca2 P2 Ca4 131.21(8) . 1_565
O9 Ca2 P2 Ca4 53.97(8) . 1_565
O8 Ca2 P2 Ca4 130.6(3) . 1_565
O3 Ca2 P2 Ca4 -136.28(17) . 1_565
O2 Ca2 P2 Ca4 -102.03(7) . 1_565
O5 Ca2 P2 Ca4 -31.85(8) . 1_565
O6 Ca2 P2 Ca4 -32.59(9) . 1_565
O4 Ca2 P2 Ca4 55.01(15) . 1_565
O1 Ca2 P2 Ca4 -157.89(7) . 1_565
P1 Ca2 P2 Ca4 -129.43(4) . 1_565
P3 Ca2 P2 Ca4 -35.30(3) . 1_565
O7 Ca2 P2 Ca3 -146.41(8) . 1_565
O9 Ca2 P2 Ca3 136.35(9) . 1_565
O8 Ca2 P2 Ca3 -147.0(3) . 1_565
O3 Ca2 P2 Ca3 -53.90(16) . 1_565
O2 Ca2 P2 Ca3 -19.65(7) . 1_565
O5 Ca2 P2 Ca3 50.53(8) . 1_565
O6 Ca2 P2 Ca3 49.79(8) . 1_565
O4 Ca2 P2 Ca3 137.39(15) . 1_565
O1 Ca2 P2 Ca3 -75.51(7) . 1_565
P1 Ca2 P2 Ca3 -47.05(3) . 1_565
P3 Ca2 P2 Ca3 47.08(3) . 1_565
O7 Ca2 P2 Ca1 -66.87(8) . .
O9 Ca2 P2 Ca1 -144.11(8) . .
O8 Ca2 P2 Ca1 -67.4(3) . .
O3 Ca2 P2 Ca1 25.64(16) . .
O2 Ca2 P2 Ca1 59.89(7) . .
O5 Ca2 P2 Ca1 130.07(9) . .
O6 Ca2 P2 Ca1 129.33(9) . .
O4 Ca2 P2 Ca1 -143.07(15) . .
O1 Ca2 P2 Ca1 4.03(7) . .
P1 Ca2 P2 Ca1 32.49(3) . .
P3 Ca2 P2 Ca1 126.62(3) . .
O7 Ca2 P2 Ca5 72.99(9) . 3_575
O9 Ca2 P2 Ca5 -4.25(10) . 3_575
O8 Ca2 P2 Ca5 72.4(3) . 3_575
O3 Ca2 P2 Ca5 165.50(18) . 3_575
O2 Ca2 P2 Ca5 -160.25(8) . 3_575
O5 Ca2 P2 Ca5 -90.07(10) . 3_575
O6 Ca2 P2 Ca5 -90.81(10) . 3_575
O4 Ca2 P2 Ca5 -3.21(15) . 3_575
O1 Ca2 P2 Ca5 143.89(9) . 3_575
P1 Ca2 P2 Ca5 172.35(6) . 3_575
P3 Ca2 P2 Ca5 -93.52(6) . 3_575
O3 Ca1 P2 O12 72.1(3) . 1_565
O12 Ca1 P2 O12 -38.6(2) 3_675 1_565
O4 Ca1 P2 O12 -177.1(2) 3_675 1_565
O1 Ca1 P2 O12 101.58(18) . 1_565
O10 Ca1 P2 O12 42.71(18) 1_565 1_565
Cl1A Ca1 P2 O12 -13.0(2) 3_675 1_565
Cl1B Ca1 P2 O12 157.3(2) 3_675 1_565
O9 Ca1 P2 O12 -107.83(18) 3_675 1_565
P1 Ca1 P2 O12 72.16(17) . 1_565
Cl1B Ca1 P2 O12 159.09(18) 1_655 1_565
Cl1A Ca1 P2 O12 -14.64(19) 1_665 1_565
O3 Ca1 P2 O4 -72.1(3) . .
O12 Ca1 P2 O4 177.3(2) 3_675 .
O4 Ca1 P2 O4 38.8(2) 3_675 .
O1 Ca1 P2 O4 -42.57(18) . .
O10 Ca1 P2 O4 -101.44(18) 1_565 .
Cl1A Ca1 P2 O4 -157.1(2) 3_675 .
Cl1B Ca1 P2 O4 13.1(2) 3_675 .
O9 Ca1 P2 O4 108.02(18) 3_675 .
P1 Ca1 P2 O4 -71.99(17) . .
Cl1B Ca1 P2 O4 14.9(2) 1_655 .
Cl1A Ca1 P2 O4 -158.79(18) 1_665 .
O3 Ca1 P2 O7 180.0(3) . 3_675
O12 Ca1 P2 O7 69.32(17) 3_675 3_675
O4 Ca1 P2 O7 -69.20(17) 3_675 3_675
O1 Ca1 P2 O7 -150.54(17) . 3_675
O10 Ca1 P2 O7 150.59(17) 1_565 3_675
Cl1A Ca1 P2 O7 94.9(2) 3_675 3_675
Cl1B Ca1 P2 O7 -94.9(2) 3_675 3_675
O9 Ca1 P2 O7 0.05(16) 3_675 3_675
P1 Ca1 P2 O7 -179.96(15) . 3_675
Cl1B Ca1 P2 O7 -93.03(17) 1_655 3_675
Cl1A Ca1 P2 O7 93.24(17) 1_665 3_675
O12 Ca1 P2 O3 -110.6(3) 3_675 .
O4 Ca1 P2 O3 110.9(3) 3_675 .
O1 Ca1 P2 O3 29.5(3) . .
O10 Ca1 P2 O3 -29.4(2) 1_565 .
Cl1A Ca1 P2 O3 -85.1(3) 3_675 .
Cl1B Ca1 P2 O3 85.2(3) 3_675 .
O9 Ca1 P2 O3 -179.9(3) 3_675 .
P1 Ca1 P2 O3 0.1(2) . .
Cl1B Ca1 P2 O3 87.0(3) 1_655 .
Cl1A Ca1 P2 O3 -86.7(3) 1_665 .
O3 Ca1 P2 Ca4 0.0(2) . 1_565
O12 Ca1 P2 Ca4 -110.60(13) 3_675 1_565
O4 Ca1 P2 Ca4 110.88(13) 3_675 1_565
O1 Ca1 P2 Ca4 29.54(12) . 1_565
O10 Ca1 P2 Ca4 -29.33(12) 1_565 1_565
Cl1A Ca1 P2 Ca4 -85.04(17) 3_675 1_565
Cl1B Ca1 P2 Ca4 85.22(17) 3_675 1_565
O9 Ca1 P2 Ca4 -179.87(11) 3_675 1_565
P1 Ca1 P2 Ca4 0.11(10) . 1_565
Cl1B Ca1 P2 Ca4 87.05(13) 1_655 1_565
Cl1A Ca1 P2 Ca4 -86.68(13) 1_665 1_565
O3 Ca1 P2 Ca3 33.2(2) . 1_565
O12 Ca1 P2 Ca3 -77.43(9) 3_675 1_565
O4 Ca1 P2 Ca3 144.06(9) 3_675 1_565
O1 Ca1 P2 Ca3 62.71(8) . 1_565
O10 Ca1 P2 Ca3 3.84(8) 1_565 1_565
Cl1A Ca1 P2 Ca3 -51.86(15) 3_675 1_565
Cl1B Ca1 P2 Ca3 118.39(15) 3_675 1_565
O9 Ca1 P2 Ca3 -146.70(8) 3_675 1_565
P1 Ca1 P2 Ca3 33.29(4) . 1_565
Cl1B Ca1 P2 Ca3 120.22(10) 1_655 1_565
Cl1A Ca1 P2 Ca3 -53.51(9) 1_665 1_565
O3 Ca1 P2 Ca2 -34.0(2) . .
O12 Ca1 P2 Ca2 -144.63(9) 3_675 .
O4 Ca1 P2 Ca2 76.86(9) 3_675 .
O1 Ca1 P2 Ca2 -4.49(8) . .
O10 Ca1 P2 Ca2 -63.36(8) 1_565 .
Cl1A Ca1 P2 Ca2 -119.06(15) 3_675 .
Cl1B Ca1 P2 Ca2 51.19(15) 3_675 .
O9 Ca1 P2 Ca2 146.10(8) 3_675 .
P1 Ca1 P2 Ca2 -33.91(4) . .
Cl1B Ca1 P2 Ca2 53.02(10) 1_655 .
Cl1A Ca1 P2 Ca2 -120.71(9) 1_665 .
O3 Ca1 P2 Ca5 179.9(3) . 3_575
O12 Ca1 P2 Ca5 69.25(11) 3_675 3_575
O4 Ca1 P2 Ca5 -69.26(11) 3_675 3_575
O1 Ca1 P2 Ca5 -150.61(9) . 3_575
O10 Ca1 P2 Ca5 150.52(9) 1_565 3_575
Cl1A Ca1 P2 Ca5 94.82(16) 3_675 3_575
Cl1B Ca1 P2 Ca5 -94.93(16) 3_675 3_575
O9 Ca1 P2 Ca5 -0.02(9) 3_675 3_575
P1 Ca1 P2 Ca5 179.97(6) . 3_575
Cl1B Ca1 P2 Ca5 -93.10(11) 1_655 3_575
Cl1A Ca1 P2 Ca5 93.17(10) 1_665 3_575
Ca4 O6 P3 O11 142.5(3) 2_655 1_565
Ca5 O6 P3 O11 -8.46(15) 2_655 1_565
Ca2 O6 P3 O11 -105.53(15) . 1_565
Ca4 O6 P3 O9 18.8(4) 2_655 2_655
Ca5 O6 P3 O9 -132.25(15) 2_655 2_655
Ca2 O6 P3 O9 130.67(15) . 2_655
Ca4 O6 P3 O5 -103.0(3) 2_655 .
Ca5 O6 P3 O5 106.01(16) 2_655 .
Ca2 O6 P3 O5 8.94(16) . .
Ca4 O6 P3 Ca5 151.0(4) 2_655 2_655
Ca2 O6 P3 Ca5 -97.07(12) . 2_655
Ca4 O6 P3 Ca3 -152.5(2) 2_655 1_565
Ca5 O6 P3 Ca3 56.45(14) 2_655 1_565
Ca2 O6 P3 Ca3 -40.62(12) . 1_565
Ca4 O6 P3 Ca2 -111.9(3) 2_655 .
Ca5 O6 P3 Ca2 97.07(12) 2_655 .
Ca4 O6 P3 Ca4 -68.6(3) 2_655 1_565
Ca5 O6 P3 Ca4 140.44(7) 2_655 1_565
Ca2 O6 P3 Ca4 43.37(14) . 1_565
Ca4 O6 P3 Ca1 66.2(3) 2_655 4_586
Ca5 O6 P3 Ca1 -84.83(10) 2_655 4_586
Ca2 O6 P3 Ca1 178.10(9) . 4_586
Ca4 O5 P3 O11 -122.7(2) 1_565 1_565
Ca3 O5 P3 O11 11.2(2) 1_565 1_565
Ca2 O5 P3 O11 104.44(18) . 1_565
Ca4 O5 P3 O6 122.3(2) 1_565 .
Ca3 O5 P3 O6 -103.76(18) 1_565 .
Ca2 O5 P3 O6 -10.6(2) . .
Ca4 O5 P3 O9 0.0(3) 1_565 2_655
Ca3 O5 P3 O9 133.97(18) 1_565 2_655
Ca2 O5 P3 O9 -132.83(18) . 2_655
Ca4 O5 P3 Ca5 179.87(14) 1_565 2_655
Ca3 O5 P3 Ca5 -46.20(17) 1_565 2_655
Ca2 O5 P3 Ca5 47.01(17) . 2_655
Ca4 O5 P3 Ca3 -133.9(3) 1_565 1_565
Ca2 O5 P3 Ca3 93.20(14) . 1_565
Ca4 O5 P3 Ca2 132.9(3) 1_565 .
Ca3 O5 P3 Ca2 -93.20(14) 1_565 .
Ca3 O5 P3 Ca4 133.9(3) 1_565 1_565
Ca2 O5 P3 Ca4 -132.9(3) . 1_565
Ca4 O5 P3 Ca1 0.0(8) 1_565 4_586
Ca3 O5 P3 Ca1 133.9(6) 1_565 4_586
Ca2 O5 P3 Ca1 -132.9(6) . 4_586
O7 Ca2 P3 O11 173.8(4) . 1_565
O9 Ca2 P3 O11 174.27(16) . 1_565
O8 Ca2 P3 O11 97.01(16) . 1_565
O3 Ca2 P3 O11 -59.01(16) . 1_565
O2 Ca2 P3 O11 11.19(16) . 1_565
O5 Ca2 P3 O11 -93.2(2) . 1_565
O6 Ca2 P3 O11 98.47(18) . 1_565
O4 Ca2 P3 O11 -114.86(16) . 1_565
O1 Ca2 P3 O11 10.35(18) . 1_565
P2 Ca2 P3 O11 -86.36(15) . 1_565
P1 Ca2 P3 O11 7.81(15) . 1_565
O7 Ca2 P3 O6 75.4(4) . .
O9 Ca2 P3 O6 75.80(16) . .
O8 Ca2 P3 O6 -1.46(16) . .
O3 Ca2 P3 O6 -157.48(16) . .
O2 Ca2 P3 O6 -87.28(16) . .
O5 Ca2 P3 O6 168.3(2) . .
O4 Ca2 P3 O6 146.67(16) . .
O1 Ca2 P3 O6 -88.12(17) . .
P2 Ca2 P3 O6 175.17(15) . .
P1 Ca2 P3 O6 -90.66(15) . .
O7 Ca2 P3 O9 -16.6(4) . 2_655
O9 Ca2 P3 O9 -16.1(2) . 2_655
O8 Ca2 P3 O9 -93.4(2) . 2_655
O3 Ca2 P3 O9 110.6(2) . 2_655
O2 Ca2 P3 O9 -179.2(2) . 2_655
O5 Ca2 P3 O9 76.4(2) . 2_655
O6 Ca2 P3 O9 -91.9(2) . 2_655
O4 Ca2 P3 O9 54.7(2) . 2_655
O1 Ca2 P3 O9 180.0(2) . 2_655
P2 Ca2 P3 O9 83.24(19) . 2_655
P1 Ca2 P3 O9 177.41(18) . 2_655
O7 Ca2 P3 O5 -93.0(4) . .
O9 Ca2 P3 O5 -92.54(18) . .
O8 Ca2 P3 O5 -169.79(18) . .
O3 Ca2 P3 O5 34.18(18) . .
O2 Ca2 P3 O5 104.39(18) . .
O6 Ca2 P3 O5 -168.3(2) . .
O4 Ca2 P3 O5 -21.66(18) . .
O1 Ca2 P3 O5 103.55(18) . .
P2 Ca2 P3 O5 6.84(16) . .
P1 Ca2 P3 O5 101.00(16) . .
O7 Ca2 P3 Ca5 130.7(3) . 2_655
O9 Ca2 P3 Ca5 131.10(8) . 2_655
O8 Ca2 P3 Ca5 53.85(8) . 2_655
O3 Ca2 P3 Ca5 -102.18(7) . 2_655
O2 Ca2 P3 Ca5 -31.97(8) . 2_655
O5 Ca2 P3 Ca5 -136.36(17) . 2_655
O6 Ca2 P3 Ca5 55.31(14) . 2_655
O4 Ca2 P3 Ca5 -158.02(7) . 2_655
O1 Ca2 P3 Ca5 -32.81(9) . 2_655
P2 Ca2 P3 Ca5 -129.52(4) . 2_655
P1 Ca2 P3 Ca5 -35.36(4) . 2_655
O7 Ca2 P3 Ca3 -146.9(4) . 1_565
O9 Ca2 P3 Ca3 -146.50(8) . 1_565
O8 Ca2 P3 Ca3 136.25(8) . 1_565
O3 Ca2 P3 Ca3 -19.78(7) . 1_565
O2 Ca2 P3 Ca3 50.42(8) . 1_565
O5 Ca2 P3 Ca3 -53.96(16) . 1_565
O6 Ca2 P3 Ca3 137.70(15) . 1_565
O4 Ca2 P3 Ca3 -75.63(7) . 1_565
O1 Ca2 P3 Ca3 49.58(9) . 1_565
P2 Ca2 P3 Ca3 -47.12(3) . 1_565
P1 Ca2 P3 Ca3 47.04(3) . 1_565
O7 Ca2 P3 Ca4 -67.3(3) . 1_565
O9 Ca2 P3 Ca4 -66.89(8) . 1_565
O8 Ca2 P3 Ca4 -144.14(8) . 1_565
O3 Ca2 P3 Ca4 59.83(7) . 1_565
O2 Ca2 P3 Ca4 130.04(9) . 1_565
O5 Ca2 P3 Ca4 25.65(16) . 1_565
O6 Ca2 P3 Ca4 -142.68(15) . 1_565
O4 Ca2 P3 Ca4 3.99(7) . 1_565
O1 Ca2 P3 Ca4 129.20(9) . 1_565
P2 Ca2 P3 Ca4 32.49(3) . 1_565
P1 Ca2 P3 Ca4 126.65(3) . 1_565
O7 Ca2 P3 Ca1 72.4(4) . 4_586
O9 Ca2 P3 Ca1 72.86(10) . 4_586
O8 Ca2 P3 Ca1 -4.40(10) . 4_586
O3 Ca2 P3 Ca1 -160.42(8) . 4_586
O2 Ca2 P3 Ca1 -90.22(10) . 4_586
O5 Ca2 P3 Ca1 165.39(18) . 4_586
O6 Ca2 P3 Ca1 -2.94(14) . 4_586
O4 Ca2 P3 Ca1 143.73(8) . 4_586
O1 Ca2 P3 Ca1 -91.06(10) . 4_586
P2 Ca2 P3 Ca1 172.23(6) . 4_586
P1 Ca2 P3 Ca1 -93.60(6) . 4_586
O2 Ca5 Cl1A Cl1A 50.9(5) 2_645 3_565
O10 Ca5 Cl1A Cl1A -16.2(4) 1_455 3_565
O1 Ca5 Cl1A Cl1A -151.2(4) 1_455 3_565
O11 Ca5 Cl1A Cl1A 123.9(4) 2_655 3_565
O6 Ca5 Cl1A Cl1A 70.3(4) 2_645 3_565
Cl1B Ca5 Cl1A Cl1A -174.8(5) . 3_565
O7 Ca5 Cl1A Cl1A -80.9(4) 1_455 3_565
P3 Ca5 Cl1A Cl1A 96.7(4) 2_645 3_565
Cl1B Ca5 Cl1A Cl1A -176.0(4) 3_575 3_565
P1 Ca5 Cl1A Cl1A 11.0(5) 2_645 3_565
O2 Ca5 Cl1A Ca1 -81.80(17) 2_645 3_675
O10 Ca5 Cl1A Ca1 -148.89(12) 1_455 3_675
O1 Ca5 Cl1A Ca1 76.06(14) 1_455 3_675
O11 Ca5 Cl1A Ca1 -8.77(11) 2_655 3_675
O6 Ca5 Cl1A Ca1 -62.36(10) 2_645 3_675
Cl1B Ca5 Cl1A Ca1 52.48(8) . 3_675
O7 Ca5 Cl1A Ca1 146.38(9) 1_455 3_675
P3 Ca5 Cl1A Ca1 -35.99(7) 2_645 3_675
Cl1B Ca5 Cl1A Ca1 51.30(9) 3_575 3_675
Cl1A Ca5 Cl1A Ca1 -132.7(5) 3_565 3_675
P1 Ca5 Cl1A Ca1 -121.69(11) 2_645 3_675
O2 Ca5 Cl1A Ca4 174.38(14) 2_645 3_565
O10 Ca5 Cl1A Ca4 107.28(11) 1_455 3_565
O1 Ca5 Cl1A Ca4 -27.76(14) 1_455 3_565
O11 Ca5 Cl1A Ca4 -112.59(10) 2_655 3_565
O6 Ca5 Cl1A Ca4 -166.18(11) 2_645 3_565
Cl1B Ca5 Cl1A Ca4 -51.34(9) . 3_565
O7 Ca5 Cl1A Ca4 42.56(10) 1_455 3_565
P3 Ca5 Cl1A Ca4 -139.81(7) 2_645 3_565
Cl1B Ca5 Cl1A Ca4 -52.53(8) 3_575 3_565
Cl1A Ca5 Cl1A Ca4 123.5(5) 3_565 3_565
P1 Ca5 Cl1A Ca4 134.48(10) 2_645 3_565
O2 Ca5 Cl1A Ca4 5.68(18) 2_645 .
O10 Ca5 Cl1A Ca4 -61.42(10) 1_455 .
O1 Ca5 Cl1A Ca4 163.54(11) 1_455 .
O11 Ca5 Cl1A Ca4 78.71(9) 2_655 .
O6 Ca5 Cl1A Ca4 25.12(8) 2_645 .
Cl1B Ca5 Cl1A Ca4 139.96(12) . .
O7 Ca5 Cl1A Ca4 -126.14(8) 1_455 .
P3 Ca5 Cl1A Ca4 51.49(5) 2_645 .
Cl1B Ca5 Cl1A Ca4 138.78(7) 3_575 .
Cl1A Ca5 Cl1A Ca4 -45.2(4) 3_565 .
P1 Ca5 Cl1A Ca4 -34.22(15) 2_645 .
O2 Ca5 Cl1A Ca5 50.9(5) 2_645 3_565
O10 Ca5 Cl1A Ca5 -16.2(4) 1_455 3_565
O1 Ca5 Cl1A Ca5 -151.2(4) 1_455 3_565
O11 Ca5 Cl1A Ca5 123.9(4) 2_655 3_565
O6 Ca5 Cl1A Ca5 70.3(4) 2_645 3_565
Cl1B Ca5 Cl1A Ca5 -174.8(5) . 3_565
O7 Ca5 Cl1A Ca5 -80.9(4) 1_455 3_565
P3 Ca5 Cl1A Ca5 96.7(4) 2_645 3_565
Cl1B Ca5 Cl1A Ca5 -176.0(4) 3_575 3_565
Cl1A Ca5 Cl1A Ca5 0 3_565 3_565
P1 Ca5 Cl1A Ca5 11.0(5) 2_645 3_565
O2 Ca5 Cl1A Ca1 88.35(17) 2_645 1_445
O10 Ca5 Cl1A Ca1 21.26(10) 1_455 1_445
O1 Ca5 Cl1A Ca1 -113.79(12) 1_455 1_445
O11 Ca5 Cl1A Ca1 161.38(9) 2_655 1_445
O6 Ca5 Cl1A Ca1 107.80(10) 2_645 1_445
Cl1B Ca5 Cl1A Ca1 -137.37(12) . 1_445
O7 Ca5 Cl1A Ca1 -43.46(9) 1_455 1_445
P3 Ca5 Cl1A Ca1 134.16(6) 2_645 1_445
Cl1B Ca5 Cl1A Ca1 -138.55(7) 3_575 1_445
Cl1A Ca5 Cl1A Ca1 37.5(4) 3_565 1_445
P1 Ca5 Cl1A Ca1 48.46(15) 2_645 1_445
O5 Ca4 Cl1A Cl1A 147.5(4) 1_545 3_565
O6 Ca4 Cl1A Cl1A -154.3(4) 2_645 3_565
O11 Ca4 Cl1A Cl1A -27.0(5) 2_645 3_565
O4 Ca4 Cl1A Cl1A 65.8(4) 1_545 3_565
O12 Ca4 Cl1A Cl1A 112.2(4) . 3_565
Cl1B Ca4 Cl1A Cl1A 3.9(4) 3_565 3_565
O8 Ca4 Cl1A Cl1A -93.4(4) 2_645 3_565
P2 Ca4 Cl1A Cl1A 90.0(4) 1_545 3_565
Cl1B Ca4 Cl1A Cl1A 3.1(4) 1_545 3_565
P3 Ca4 Cl1A Cl1A 179.1(4) 1_545 3_565
O5 Ca4 Cl1A Ca1 14.39(15) 1_545 3_675
O6 Ca4 Cl1A Ca1 72.65(11) 2_645 3_675
O11 Ca4 Cl1A Ca1 -160.06(14) 2_645 3_675
O4 Ca4 Cl1A Ca1 -67.28(10) 1_545 3_675
O12 Ca4 Cl1A Ca1 -20.85(9) . 3_675
Cl1B Ca4 Cl1A Ca1 -129.20(7) 3_565 3_675
Cl1A Ca4 Cl1A Ca1 -133.1(4) 3_565 3_675
O8 Ca4 Cl1A Ca1 133.56(8) 2_645 3_675
P2 Ca4 Cl1A Ca1 -43.12(6) 1_545 3_675
Cl1B Ca4 Cl1A Ca1 -130.03(9) 1_545 3_675
P3 Ca4 Cl1A Ca1 46.05(11) 1_545 3_675
O5 Ca4 Cl1A Ca5 -87.05(13) 1_545 .
O6 Ca4 Cl1A Ca5 -28.79(10) 2_645 .
O11 Ca4 Cl1A Ca5 98.49(15) 2_645 .
O4 Ca4 Cl1A Ca5 -168.72(9) 1_545 .
O12 Ca4 Cl1A Ca5 -122.29(11) . .
Cl1B Ca4 Cl1A Ca5 129.36(7) 3_565 .
Cl1A Ca4 Cl1A Ca5 125.5(4) 3_565 .
O8 Ca4 Cl1A Ca5 32.12(9) 2_645 .
P2 Ca4 Cl1A Ca5 -144.56(6) 1_545 .
Cl1B Ca4 Cl1A Ca5 128.53(8) 1_545 .
P3 Ca4 Cl1A Ca5 -55.39(10) 1_545 .
O5 Ca4 Cl1A Ca4 147.5(4) 1_545 3_565
O6 Ca4 Cl1A Ca4 -154.3(4) 2_645 3_565
O11 Ca4 Cl1A Ca4 -27.0(5) 2_645 3_565
O4 Ca4 Cl1A Ca4 65.8(4) 1_545 3_565
O12 Ca4 Cl1A Ca4 112.2(4) . 3_565
Cl1B Ca4 Cl1A Ca4 3.9(4) 3_565 3_565
Cl1A Ca4 Cl1A Ca4 0 3_565 3_565
O8 Ca4 Cl1A Ca4 -93.4(4) 2_645 3_565
P2 Ca4 Cl1A Ca4 90.0(4) 1_545 3_565
Cl1B Ca4 Cl1A Ca4 3.1(4) 1_545 3_565
P3 Ca4 Cl1A Ca4 179.1(4) 1_545 3_565
O5 Ca4 Cl1A Ca5 102.60(12) 1_545 3_565
O6 Ca4 Cl1A Ca5 160.85(11) 2_645 3_565
O11 Ca4 Cl1A Ca5 -71.86(15) 2_645 3_565
O4 Ca4 Cl1A Ca5 20.93(9) 1_545 3_565
O12 Ca4 Cl1A Ca5 67.36(9) . 3_565
Cl1B Ca4 Cl1A Ca5 -40.99(7) 3_565 3_565
Cl1A Ca4 Cl1A Ca5 -44.9(4) 3_565 3_565
O8 Ca4 Cl1A Ca5 -138.23(8) 2_645 3_565
P2 Ca4 Cl1A Ca5 45.09(5) 1_545 3_565
Cl1B Ca4 Cl1A Ca5 -41.82(5) 1_545 3_565
P3 Ca4 Cl1A Ca5 134.26(6) 1_545 3_565
O5 Ca4 Cl1A Ca1 -174.18(11) 1_545 1_445
O6 Ca4 Cl1A Ca1 -115.93(11) 2_645 1_445
O11 Ca4 Cl1A Ca1 11.36(16) 2_645 1_445
O4 Ca4 Cl1A Ca1 104.14(9) 1_545 1_445
O12 Ca4 Cl1A Ca1 150.58(11) . 1_445
Cl1B Ca4 Cl1A Ca1 42.23(7) 3_565 1_445
Cl1A Ca4 Cl1A Ca1 38.3(4) 3_565 1_445
O8 Ca4 Cl1A Ca1 -55.02(8) 2_645 1_445
P2 Ca4 Cl1A Ca1 128.30(5) 1_545 1_445
Cl1B Ca4 Cl1A Ca1 41.39(5) 1_545 1_445
P3 Ca4 Cl1A Ca1 -142.52(5) 1_545 1_445
O2 Ca5 Cl1B Cl1B -39.7(6) 2_645 3_575
O10 Ca5 Cl1B Cl1B 158.8(5) 1_455 3_575
O1 Ca5 Cl1B Cl1B 24.8(5) 1_455 3_575
O11 Ca5 Cl1B Cl1B -62.2(5) 2_655 3_575
O6 Ca5 Cl1B Cl1B -115.1(5) 2_645 3_575
Cl1A Ca5 Cl1B Cl1B -174.5(6) . 3_575
O7 Ca5 Cl1B Cl1B 89.5(5) 1_455 3_575
P3 Ca5 Cl1B Cl1B -88.0(5) 2_645 3_575
Cl1A Ca5 Cl1B Cl1B -175.8(5) 3_565 3_575
P1 Ca5 Cl1B Cl1B -0.1(6) 2_645 3_575
O2 Ca5 Cl1B Ca4 -173.93(14) 2_645 3_565
O10 Ca5 Cl1B Ca4 24.58(15) 1_455 3_565
O1 Ca5 Cl1B Ca4 -109.43(11) 1_455 3_565
O11 Ca5 Cl1B Ca4 163.61(11) 2_655 3_565
O6 Ca5 Cl1B Ca4 110.70(10) 2_645 3_565
Cl1A Ca5 Cl1B Ca4 51.35(9) . 3_565
O7 Ca5 Cl1B Ca4 -44.70(10) 1_455 3_565
P3 Ca5 Cl1B Ca4 137.81(7) 2_645 3_565
Cl1B Ca5 Cl1B Ca4 -134.2(6) 3_575 3_565
Cl1A Ca5 Cl1B Ca4 50.04(8) 3_565 3_565
P1 Ca5 Cl1B Ca4 -134.26(10) 2_645 3_565
O2 Ca5 Cl1B Ca1 84.65(17) 2_645 3_675
O10 Ca5 Cl1B Ca1 -76.84(14) 1_455 3_675
O1 Ca5 Cl1B Ca1 149.15(12) 1_455 3_675
O11 Ca5 Cl1B Ca1 62.19(10) 2_655 3_675
O6 Ca5 Cl1B Ca1 9.27(11) 2_645 3_675
Cl1A Ca5 Cl1B Ca1 -50.08(8) . 3_675
O7 Ca5 Cl1B Ca1 -146.12(9) 1_455 3_675
P3 Ca5 Cl1B Ca1 36.39(7) 2_645 3_675
Cl1B Ca5 Cl1B Ca1 124.4(6) 3_575 3_675
Cl1A Ca5 Cl1B Ca1 -51.38(8) 3_565 3_675
P1 Ca5 Cl1B Ca1 124.31(11) 2_645 3_675
O2 Ca5 Cl1B Ca1 -85.96(17) 2_645 1_455
O10 Ca5 Cl1B Ca1 112.55(12) 1_455 1_455
O1 Ca5 Cl1B Ca1 -21.46(10) 1_455 1_455
O11 Ca5 Cl1B Ca1 -108.42(10) 2_655 1_455
O6 Ca5 Cl1B Ca1 -161.34(9) 2_645 1_455
Cl1A Ca5 Cl1B Ca1 139.31(13) . 1_455
O7 Ca5 Cl1B Ca1 43.27(9) 1_455 1_455
P3 Ca5 Cl1B Ca1 -134.22(6) 2_645 1_455
Cl1B Ca5 Cl1B Ca1 -46.2(5) 3_575 1_455
Cl1A Ca5 Cl1B Ca1 138.01(7) 3_565 1_455
P1 Ca5 Cl1B Ca1 -46.30(16) 2_645 1_455
O2 Ca5 Cl1B Ca5 -39.7(6) 2_645 3_575
O10 Ca5 Cl1B Ca5 158.8(5) 1_455 3_575
O1 Ca5 Cl1B Ca5 24.8(5) 1_455 3_575
O11 Ca5 Cl1B Ca5 -62.2(5) 2_655 3_575
O6 Ca5 Cl1B Ca5 -115.1(5) 2_645 3_575
Cl1A Ca5 Cl1B Ca5 -174.5(6) . 3_575
O7 Ca5 Cl1B Ca5 89.5(5) 1_455 3_575
P3 Ca5 Cl1B Ca5 -88.0(5) 2_645 3_575
Cl1B Ca5 Cl1B Ca5 0 3_575 3_575
Cl1A Ca5 Cl1B Ca5 -175.8(5) 3_565 3_575
P1 Ca5 Cl1B Ca5 -0.1(6) 2_645 3_575
O2 Ca5 Cl1B Ca4 -2.00(18) 2_645 1_565
O10 Ca5 Cl1B Ca4 -163.49(11) 1_455 1_565
O1 Ca5 Cl1B Ca4 62.50(10) 1_455 1_565
O11 Ca5 Cl1B Ca4 -24.46(8) 2_655 1_565
O6 Ca5 Cl1B Ca4 -77.37(9) 2_645 1_565
Cl1A Ca5 Cl1B Ca4 -136.73(12) . 1_565
O7 Ca5 Cl1B Ca4 127.23(8) 1_455 1_565
P3 Ca5 Cl1B Ca4 -50.26(5) 2_645 1_565
Cl1B Ca5 Cl1B Ca4 37.7(5) 3_575 1_565
Cl1A Ca5 Cl1B Ca4 -138.03(7) 3_565 1_565
P1 Ca5 Cl1B Ca4 37.67(16) 2_645 1_565
